 
data_4656 
 
_audit_creation_method            SHELXL-97 
_chemical_name_systematic 
; 
 ? 
; 
_chemical_name_common             ? 
_chemical_melting_point           ? 
_chemical_formula_moiety          ? 
_chemical_formula_sum 
 'Al0.70 As4 Ca0.10 Cu5.10 Fe0.20 K2 Na0.90 O18' 
_chemical_formula_weight          1044.69 
 
loop_ 
 _atom_type_symbol 
 _atom_type_description 
 _atom_type_scat_dispersion_real 
 _atom_type_scat_dispersion_imag 
 _atom_type_scat_source 
 'As'  'As'   0.0499   2.0058 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Cu'  'Cu'   0.3201   1.2651 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'K'  'K'   0.2009   0.2494 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Na'  'Na'   0.0362   0.0249 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'O'  'O'   0.0106   0.0060 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Al'  'Al'   0.0645   0.0514 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Fe'  'Fe'   0.3463   0.8444 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Ca'  'Ca'   0.2262   0.3064 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 
_symmetry_cell_setting            ? 
_symmetry_space_group_name_H-M    ? 
 
loop_ 
 _symmetry_equiv_pos_as_xyz 
 'x, y, z' 
 '-x, -y, -z' 
 
_cell_length_a                    5.0904(11) 
_cell_length_b                    9.0778(14) 
_cell_length_c                    9.658(2) 
_cell_angle_alpha                 110.334(17) 
_cell_angle_beta                  102.461(19) 
_cell_angle_gamma                 92.788(15) 
_cell_volume                      404.88(14) 
_cell_formula_units_Z             1 
_cell_measurement_temperature     293(2) 
_cell_measurement_reflns_used     ? 
_cell_measurement_theta_min       ? 
_cell_measurement_theta_max       ? 
 
_exptl_crystal_description        ? 
_exptl_crystal_colour             ? 
_exptl_crystal_size_max           ? 
_exptl_crystal_size_mid           ? 
_exptl_crystal_size_min           ? 
_exptl_crystal_density_meas       ? 
_exptl_crystal_density_diffrn     4.285 
_exptl_crystal_density_method     'not measured' 
_exptl_crystal_F_000              488 
_exptl_absorpt_coefficient_mu     15.579 
_exptl_absorpt_correction_type    ? 
_exptl_absorpt_correction_T_min   ? 
_exptl_absorpt_correction_T_max   ? 
_exptl_absorpt_process_details    ? 
 
_exptl_special_details 
; 
 ? 
; 
 
_diffrn_ambient_temperature       293(2) 
_diffrn_radiation_wavelength      0.71073 
_diffrn_radiation_type            MoK\a 
_diffrn_radiation_source          'fine-focus sealed tube' 
_diffrn_radiation_monochromator   graphite 
_diffrn_measurement_device_type   ? 
_diffrn_measurement_method        ? 
_diffrn_detector_area_resol_mean  ? 
_diffrn_standards_number          ? 
_diffrn_standards_interval_count  ? 
_diffrn_standards_interval_time   ? 
_diffrn_standards_decay_%         ? 
_diffrn_reflns_number             6270 
_diffrn_reflns_av_R_equivalents   0.1654 
_diffrn_reflns_av_sigmaI/netI     0.2130 
_diffrn_reflns_limit_h_min        -6 
_diffrn_reflns_limit_h_max        6 
_diffrn_reflns_limit_k_min        -12 
_diffrn_reflns_limit_k_max        12 
_diffrn_reflns_limit_l_min        -12 
_diffrn_reflns_limit_l_max        12 
_diffrn_reflns_theta_min          3.92 
_diffrn_reflns_theta_max          28.28 
_reflns_number_total              2014 
_reflns_number_gt                 1046 
_reflns_threshold_expression      >2sigma(I) 
 
_computing_data_collection        ? 
_computing_cell_refinement        ? 
_computing_data_reduction         ? 
_computing_structure_solution     'SHELXS-97 (Sheldrick, 1990)' 
_computing_structure_refinement   'SHELXL-97 (Sheldrick, 1997)' 
_computing_molecular_graphics     ? 
_computing_publication_material   ? 
 
_refine_special_details 
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
; 
 
_refine_ls_structure_factor_coef  Fsqd  
_refine_ls_matrix_type            full 
_refine_ls_weighting_scheme       calc  
_refine_ls_weighting_details 
 'calc w=1/[σ²(Fo²)+(0.0908P)²+0.0000P] where P=(Fo²+2Fc²)/3' 
_atom_sites_solution_primary      direct 
_atom_sites_solution_secondary    difmap 
_atom_sites_solution_hydrogens    geom 
_refine_ls_hydrogen_treatment     mixed 
_refine_ls_extinction_method      none 
_refine_ls_extinction_coef        ? 
_refine_ls_number_reflns          2014 
_refine_ls_number_parameters      137 
_refine_ls_number_restraints      0 
_refine_ls_R_factor_all           0.1708 
_refine_ls_R_factor_gt            0.0826 
_refine_ls_wR_factor_ref          0.2187 
_refine_ls_wR_factor_gt           0.1707 
_refine_ls_goodness_of_fit_ref    0.946 
_refine_ls_restrained_S_all       0.946 
_refine_ls_shift/su_max           0.000 
_refine_ls_shift/su_mean          0.000 
 
loop_ 
 _atom_site_label 
 _atom_site_type_symbol 
 _atom_site_fract_x 
 _atom_site_fract_y 
 _atom_site_fract_z 
 _atom_site_U_iso_or_equiv 
 _atom_site_adp_type 
 _atom_site_occupancy 
 _atom_site_symmetry_multiplicity 
 _atom_site_calc_flag 
 _atom_site_refinement_flags 
 _atom_site_disorder_assembly 
 _atom_site_disorder_group 
K1 K 0.2685(9) 0.2183(6) 0.5772(5) 0.0316(12) Uani 1 1 d . . . 
Na1 Na 0.5000 0.5000 0.0000 0.059(4) Uani 0.90 2 d SP . . 
Ca1 Ca 0.5000 0.5000 0.0000 0.059(4) Uani 0.10 2 d SP . . 
As1 As -0.0357(4) 0.2662(2) 0.8885(2) 0.0125(5) Uani 1 1 d . . . 
As2 As 0.6896(4) 0.3059(2) 0.3680(2) 0.0145(5) Uani 1 1 d . . . 
Cu1 Cu 0.8165(5) 0.5162(3) 0.7361(3) 0.0178(6) Uani 1 1 d . . . 
Cu2 Cu 0.4321(4) 0.0843(3) 0.9020(3) 0.0166(6) Uani 1 1 d . . . 
Cu Cu 0.8937(6) 0.8864(3) 0.8433(3) 0.0159(7) Uani 0.55 1 d P . . 
Al Al 0.8937(6) 0.8864(3) 0.8433(3) 0.0159(7) Uani 0.35 1 d P . . 
Fe Fe 0.8937(6) 0.8864(3) 0.8433(3) 0.0159(7) Uani 0.10 1 d P . . 
O1 O -0.018(3) 0.2734(16) 0.3104(16) 0.022(3) Uani 1 1 d . . . 
O2 O 0.062(3) 0.0946(15) 0.7841(15) 0.023(3) Uani 1 1 d . . . 
O3 O 0.155(2) 0.3014(16) 0.0681(14) 0.021(3) Uani 1 1 d . . . 
O4 O 0.216(3) 0.6682(15) 0.4484(15) 0.023(3) Uani 1 1 d . . . 
O5 O 0.073(2) 0.4141(16) 0.8431(16) 0.021(3) Uani 1 1 d . . . 
O6 O 0.457(3) 0.1428(14) 0.2857(15) 0.020(3) Uani 1 1 d . . . 
O7 O 0.237(2) -0.0352(14) 0.9915(13) 0.011(3) Uiso 1 1 d . . . 
O8 O 0.436(3) 0.5424(15) 0.6709(15) 0.021(3) Uani 1 1 d . . . 
O9 O 0.626(3) 0.2553(14) 0.8611(13) 0.015(3) Uani 1 1 d . . . 
 
 
_geom_special_details 
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
; 
 
loop_ 
 _geom_bond_atom_site_label_1 
 _geom_bond_atom_site_label_2 
 _geom_bond_distance 
 _geom_bond_site_symmetry_2 
 _geom_bond_publ_flag 
K1 O4 2.714(15) 2_566 ? 
K1 O8 2.788(14) . ? 
K1 O9 2.844(13) . ? 
K1 O4 2.864(15) 2_666 ? 
K1 O1 2.891(14) . ? 
K1 O2 2.951(15) . ? 
K1 O5 2.976(15) . ? 
K1 O6 3.035(13) . ? 
K1 Cu1 3.462(5) . ? 
K1 As2 3.482(5) . ? 
K1 As2 3.489(5) 1_455 ? 
K1 As1 3.577(5) . ? 
K1 O2 3.632(14) 2_556 ? 
K1 Cu2 3.694(5) . ? 
K1 Fe 3.724(6) 2_666 ? 
K1 Al 3.724(6) 2_666 ? 
K1 Cu 3.724(6) 2_666 ? 
K1 Cu1 3.769(6) 1_455 ? 
K1 Ca1 3.870(5) 1_556 ? 
K1 Na1 3.870(5) 1_556 ? 
Na1 O5 2.287(12) 2_666 ? 
Na1 O5 2.287(12) 1_554 ? 
Na1 O9 2.363(12) 2_666 ? 
Na1 O9 2.363(12) 1_554 ? 
Na1 O3 2.790(13) 2_665 ? 
Na1 O3 2.790(13) . ? 
Na1 As1 3.1115(19) 2_666 ? 
Na1 As1 3.1115(19) 1_554 ? 
Na1 O8 3.282(12) 1_554 ? 
Na1 O8 3.282(12) 2_666 ? 
Na1 Cu1 3.335(2) 1_554 ? 
Na1 Cu1 3.335(2) 2_666 ? 
Na1 As1 3.354(2) 1_654 ? 
Na1 As1 3.354(2) 2_566 ? 
Na1 Cu2 3.537(2) 2_666 ? 
Na1 Cu2 3.537(2) 1_554 ? 
Na1 O5 3.565(13) 1_654 ? 
Na1 O5 3.565(13) 2_566 ? 
Na1 O2 3.837(13) 2_666 ? 
Na1 O2 3.837(13) 1_554 ? 
As1 O5 1.656(12) . ? 
As1 O9 1.679(13) 1_455 ? 
As1 O2 1.701(13) . ? 
As1 O3 1.705(13) 1_556 ? 
As1 Cu2 2.968(3) . ? 
As1 Ca1 3.1115(19) 1_556 ? 
As1 Na1 3.1115(19) 1_556 ? 
As1 Cu1 3.146(3) 1_455 ? 
As1 Cu2 3.155(3) 1_455 ? 
As1 Cu 3.306(3) 2_667 ? 
As1 Cu 3.312(3) 1_445 ? 
As1 Ca1 3.354(2) 1_456 ? 
As2 O4 1.662(13) 2_666 ? 
As2 O8 1.670(13) 2_666 ? 
As2 O6 1.682(12) . ? 
As2 O1 1.704(13) 1_655 ? 
As2 Cu 3.230(4) 2_666 ? 
As2 Cu1 3.267(3) 2_666 ? 
As2 Cu1 3.297(3) . ? 
As2 Cu 3.386(4) 2_766 ? 
As2 Cu1 3.430(3) 2_766 ? 
As2 K1 3.489(5) 1_655 ? 
As2 Cu2 3.522(3) 2_656 ? 
Cu1 O4 1.943(13) 2_666 ? 
Cu1 O8 1.956(13) . ? 
Cu1 O5 1.956(12) 1_655 ? 
Cu1 O3 2.005(13) 2_666 ? 
Cu1 O1 2.345(13) 2_666 ? 
Cu1 Cu 3.130(4) . ? 
Cu1 As1 3.146(3) 1_655 ? 
Cu1 O9 3.206(12) . ? 
Cu1 As2 3.267(3) 2_666 ? 
Cu1 Ca1 3.335(2) 1_556 ? 
Cu1 Na1 3.335(2) 1_556 ? 
Cu1 O8 3.360(14) 1_655 ? 
Cu1 As1 3.370(3) 2_667 ? 
Cu1 As2 3.430(3) 2_766 ? 
Cu1 O6 3.509(13) 2_666 ? 
Cu1 O8 3.700(13) 2_666 ? 
Cu2 O7 1.932(12) 2_657 ? 
Cu2 O7 1.955(12) . ? 
Cu2 O9 1.996(12) . ? 
Cu2 O2 2.003(14) . ? 
Cu2 O6 2.410(13) 2_656 ? 
Cu2 O3 2.739(13) 1_556 ? 
Cu2 Cu2 2.819(5) 2_657 ? 
Cu2 Fe 3.033(4) 1_445 ? 
Cu2 Al 3.033(4) 1_445 ? 
Cu2 Cu 3.033(4) 1_445 ? 
Cu2 Fe 3.057(4) 1_545 ? 
Cu2 Al 3.057(4) 1_545 ? 
Cu2 Cu 3.057(4) 1_545 ? 
Cu2 As1 3.155(3) 1_655 ? 
Cu2 Fe 3.196(4) 2_667 ? 
Cu2 Al 3.196(4) 2_667 ? 
Cu2 Cu 3.196(4) 2_667 ? 
Cu2 O1 3.470(14) 2_556 ? 
Cu2 As2 3.522(3) 2_656 ? 
Cu O6 1.891(14) 2_666 ? 
Cu O1 1.925(14) 2_666 ? 
Cu O7 1.925(12) 1_665 ? 
Cu O7 1.965(12) 2_667 ? 
Cu O3 2.183(15) 2_666 ? 
Cu O2 2.333(14) 1_665 ? 
Cu Fe 2.935(6) 2_777 ? 
Cu Al 2.935(6) 2_777 ? 
Cu Cu 2.935(6) 2_777 ? 
Cu Cu2 3.033(4) 1_665 ? 
Cu Cu2 3.057(4) 1_565 ? 
Cu Cu2 3.196(4) 2_667 ? 
Cu As2 3.230(4) 2_666 ? 
Cu As1 3.306(3) 2_667 ? 
Cu As1 3.312(3) 1_665 ? 
Cu As2 3.386(4) 2_766 ? 
Cu O8 3.458(13) . ? 
Cu O2 3.499(14) 2_667 ? 
Cu O3 3.641(14) 1_666 ? 
O1 As2 1.704(13) 1_455 ? 
O1 Fe 1.925(14) 2_666 ? 
O1 Al 1.925(14) 2_666 ? 
O1 Cu 1.925(14) 2_666 ? 
O1 Cu1 2.345(12) 2_666 ? 
O1 Cu2 3.470(14) 2_556 ? 
O1 Cu2 4.051(14) 1_454 ? 
O1 Cu1 4.225(14) 1_455 ? 
O1 Cu 4.383(13) 2_566 ? 
O1 Cu 4.567(15) 1_444 ? 
O1 Na1 4.566(13) 1_455 ? 
O2 Fe 2.333(14) 1_445 ? 
O2 Al 2.333(14) 1_445 ? 
O2 Cu 2.333(14) 1_445 ? 
O2 Cu 3.499(14) 2_667 ? 
O2 K1 3.632(14) 2_556 ? 
O2 Cu2 3.637(14) 1_455 ? 
O2 Na1 3.837(13) 1_556 ? 
O2 Cu1 4.229(13) 1_455 ? 
O2 Cu2 4.348(13) 2_657 ? 
O3 As1 1.705(12) 1_554 ? 
O3 Cu1 2.005(13) 2_666 ? 
O3 Fe 2.183(14) 2_666 ? 
O3 Al 2.183(14) 2_666 ? 
O3 Cu 2.183(14) 2_666 ? 
O3 Cu2 2.739(13) 1_554 ? 
O3 Cu 3.641(14) 1_444 ? 
O3 Cu2 3.813(13) 1_454 ? 
O3 Na1 3.905(13) 1_455 ? 
O3 Cu2 4.234(14) 2_656 ? 
O4 As2 1.662(13) 2_666 ? 
O4 Cu1 1.943(13) 2_666 ? 
O4 K1 2.714(15) 2_566 ? 
O4 K1 2.864(15) 2_666 ? 
O4 Cu1 4.312(13) 1_455 ? 
O4 Cu 4.351(14) 1_455 ? 
O4 Cu2 4.549(13) 1_565 ? 
O4 K1 4.687(14) 1_565 ? 
O5 Cu1 1.956(12) 1_455 ? 
O5 Ca1 2.287(12) 1_556 ? 
O5 Na1 2.287(12) 1_556 ? 
O5 Na1 3.565(13) 1_456 ? 
O5 Cu1 3.798(14) 2_667 ? 
O5 K1 4.253(13) 1_455 ? 
O5 Cu 4.425(13) 1_455 ? 
O5 Cu2 4.578(12) 1_455 ? 
O6 Fe 1.891(14) 2_666 ? 
O6 Al 1.891(14) 2_666 ? 
O6 Cu 1.891(14) 2_666 ? 
O6 Cu2 2.410(13) 2_656 ? 
O6 Cu1 3.509(13) 2_666 ? 
O6 Cu2 3.528(13) 1_554 ? 
O6 Cu 3.764(13) 2_766 ? 
O6 K1 4.137(14) 2_656 ? 
O6 K1 4.338(14) 1_655 ? 
O6 Cu 4.364(13) 1_444 ? 
O7 Fe 1.925(12) 1_445 ? 
O7 Al 1.925(12) 1_445 ? 
O7 Cu 1.925(12) 1_445 ? 
O7 Cu2 1.932(12) 2_657 ? 
O7 Fe 1.965(12) 2_667 ? 
O7 Al 1.965(12) 2_667 ? 
O7 Cu 1.965(12) 2_667 ? 
O7 Cu2 3.814(12) 2_557 ? 
O7 Cu 3.913(12) 1_545 ? 
O7 Cu1 4.141(12) 1_445 ? 
O7 Cu2 4.275(12) 1_455 ? 
O8 As2 1.670(13) 2_666 ? 
O8 Na1 3.282(12) 1_556 ? 
O8 Cu1 3.360(13) 1_455 ? 
O8 Cu1 3.700(13) 2_666 ? 
O8 K1 4.192(13) 2_666 ? 
O8 Cu2 4.221(14) 2_667 ? 
O8 Cu 4.400(14) 1_455 ? 
O8 Cu2 4.645(14) 1_565 ? 
O8 K1 4.898(13) 2_566 ? 
O9 As1 1.679(13) 1_655 ? 
O9 Ca1 2.363(12) 1_556 ? 
O9 Na1 2.363(12) 1_556 ? 
O9 Cu 3.640(12) 1_545 ? 
O9 Cu 3.954(12) 2_767 ? 
O9 Cu1 4.068(12) 2_767 ? 
O9 Cu2 4.445(13) 1_655 ? 
O9 Cu2 4.464(11) 2_657 ? 
O9 Na1 4.575(13) 1_656 ? 
 
loop_ 
 _geom_angle_atom_site_label_1 
 _geom_angle_atom_site_label_2 
 _geom_angle_atom_site_label_3 
 _geom_angle 
 _geom_angle_site_symmetry_1 
 _geom_angle_site_symmetry_3 
 _geom_angle_publ_flag 
O4 K1 O8 78.8(4) 2_566 . ? 
O4 K1 O9 123.5(4) 2_566 . ? 
O8 K1 O9 82.9(4) . . ? 
O4 K1 O4 131.7(5) 2_566 2_666 ? 
O8 K1 O4 59.2(4) . 2_666 ? 
O9 K1 O4 76.5(4) . 2_666 ? 
O4 K1 O1 55.9(4) 2_566 . ? 
O8 K1 O1 80.6(4) . . ? 
O9 K1 O1 163.2(4) . . ? 
O4 K1 O1 92.2(4) 2_666 . ? 
O4 K1 O2 82.5(4) 2_566 . ? 
O8 K1 O2 119.5(4) . . ? 
O9 K1 O2 61.6(4) . . ? 
O4 K1 O2 137.3(4) 2_666 . ? 
O1 K1 O2 130.5(4) . . ? 
O4 K1 O5 56.4(4) 2_566 . ? 
O8 K1 O5 66.5(4) . . ? 
O9 K1 O5 67.2(3) . . ? 
O4 K1 O5 117.0(4) 2_666 . ? 
O1 K1 O5 108.5(4) . . ? 
O2 K1 O5 55.3(4) . . ? 
O4 K1 O6 111.4(4) 2_566 . ? 
O8 K1 O6 92.9(4) . . ? 
O9 K1 O6 122.5(4) . . ? 
O4 K1 O6 53.7(4) 2_666 . ? 
O1 K1 O6 55.5(4) . . ? 
O2 K1 O6 147.1(4) . . ? 
O5 K1 O6 157.0(4) . . ? 
O4 K1 Cu1 112.8(3) 2_566 . ? 
O8 K1 Cu1 34.4(3) . . ? 
O9 K1 Cu1 60.2(3) . . ? 
O4 K1 Cu1 34.1(3) 2_666 . ? 
O1 K1 Cu1 103.6(3) . . ? 
O2 K1 Cu1 117.7(3) . . ? 
O5 K1 Cu1 82.9(3) . . ? 
O6 K1 Cu1 85.3(3) . . ? 
O4 K1 As2 116.0(3) 2_566 . ? 
O8 K1 As2 67.2(3) . . ? 
O9 K1 As2 104.5(3) . . ? 
O4 K1 As2 28.3(3) 2_666 . ? 
O1 K1 As2 65.9(3) . . ? 
O2 K1 As2 161.5(3) . . ? 
O5 K1 As2 133.6(3) . . ? 
O6 K1 As2 28.9(2) . . ? 
Cu1 K1 As2 56.69(9) . . ? 
O4 K1 As2 27.6(3) 2_566 1_455 ? 
O8 K1 As2 83.2(3) . 1_455 ? 
O9 K1 As2 150.5(3) . 1_455 ? 
O4 K1 As2 117.3(3) 2_666 1_455 ? 
O1 K1 As2 29.1(3) . 1_455 ? 
O2 K1 As2 104.0(3) . 1_455 ? 
O5 K1 As2 83.4(3) . 1_455 ? 
O6 K1 As2 84.0(3) . 1_455 ? 
Cu1 K1 As2 115.63(15) . 1_455 ? 
As2 K1 As2 93.80(12) . 1_455 ? 
O4 K1 As1 64.8(3) 2_566 . ? 
O8 K1 As1 93.3(3) . . ? 
O9 K1 As1 63.5(3) . . ? 
O4 K1 As1 134.3(3) 2_666 . ? 
O1 K1 As1 120.5(3) . . ? 
O2 K1 As1 28.2(3) . . ? 
O5 K1 As1 27.4(2) . . ? 
O6 K1 As1 171.9(3) . . ? 
Cu1 K1 As1 102.78(14) . . ? 
As2 K1 As1 158.95(17) . . ? 
As2 K1 As1 91.52(12) 1_455 . ? 
O4 K1 O2 84.8(4) 2_566 2_556 ? 
O8 K1 O2 135.0(4) . 2_556 ? 
O9 K1 O2 139.3(4) . 2_556 ? 
O4 K1 O2 107.6(4) 2_666 2_556 ? 
O1 K1 O2 55.9(4) . 2_556 ? 
O2 K1 O2 99.2(3) . 2_556 ? 
O5 K1 O2 133.6(4) . 2_556 ? 
O6 K1 O2 55.0(3) . 2_556 ? 
Cu1 K1 O2 140.3(3) . 2_556 ? 
As2 K1 O2 83.7(3) . 2_556 ? 
As2 K1 O2 64.6(2) 1_455 2_556 ? 
As1 K1 O2 116.9(3) . 2_556 ? 
O4 K1 Cu2 112.2(3) 2_566 . ? 
O8 K1 Cu2 110.8(3) . . ? 
O9 K1 Cu2 32.4(2) . . ? 
O4 K1 Cu2 104.7(3) 2_666 . ? 
O1 K1 Cu2 162.7(3) . . ? 
O2 K1 Cu2 32.7(3) . . ? 
O5 K1 Cu2 67.0(2) . . ? 
O6 K1 Cu2 133.4(3) . . ? 
Cu1 K1 Cu2 92.51(12) . . ? 
As2 K1 Cu2 129.82(15) . . ? 
As2 K1 Cu2 136.38(15) 1_455 . ? 
As1 K1 Cu2 48.16(8) . . ? 
O2 K1 Cu2 114.2(3) 2_556 . ? 
O4 K1 Fe 83.4(3) 2_566 2_666 ? 
O8 K1 Fe 99.2(3) . 2_666 ? 
O9 K1 Fe 152.5(3) . 2_666 ? 
O4 K1 Fe 81.1(3) 2_666 2_666 ? 
O1 K1 Fe 30.7(3) . 2_666 ? 
O2 K1 Fe 134.9(3) . 2_666 ? 
O5 K1 Fe 138.7(3) . 2_666 ? 
O6 K1 Fe 30.4(3) . 2_666 ? 
Cu1 K1 Fe 107.27(13) . 2_666 ? 
As2 K1 Fe 53.13(9) . 2_666 ? 
As2 K1 Fe 55.87(9) 1_455 2_666 ? 
As1 K1 Fe 142.82(15) . 2_666 ? 
O2 K1 Fe 37.0(2) 2_556 2_666 ? 
Cu2 K1 Fe 148.07(17) . 2_666 ? 
O4 K1 Al 83.4(3) 2_566 2_666 ? 
O8 K1 Al 99.2(3) . 2_666 ? 
O9 K1 Al 152.5(3) . 2_666 ? 
O4 K1 Al 81.1(3) 2_666 2_666 ? 
O1 K1 Al 30.7(3) . 2_666 ? 
O2 K1 Al 134.9(3) . 2_666 ? 
O5 K1 Al 138.7(3) . 2_666 ? 
O6 K1 Al 30.4(3) . 2_666 ? 
Cu1 K1 Al 107.27(13) . 2_666 ? 
As2 K1 Al 53.13(9) . 2_666 ? 
As2 K1 Al 55.87(9) 1_455 2_666 ? 
As1 K1 Al 142.82(15) . 2_666 ? 
O2 K1 Al 37.0(2) 2_556 2_666 ? 
Cu2 K1 Al 148.07(17) . 2_666 ? 
Fe K1 Al 0.0 2_666 2_666 ? 
O4 K1 Cu 83.4(3) 2_566 2_666 ? 
O8 K1 Cu 99.2(3) . 2_666 ? 
O9 K1 Cu 152.5(3) . 2_666 ? 
O4 K1 Cu 81.1(3) 2_666 2_666 ? 
O1 K1 Cu 30.7(3) . 2_666 ? 
O2 K1 Cu 134.9(3) . 2_666 ? 
O5 K1 Cu 138.7(3) . 2_666 ? 
O6 K1 Cu 30.4(3) . 2_666 ? 
Cu1 K1 Cu 107.27(13) . 2_666 ? 
As2 K1 Cu 53.13(9) . 2_666 ? 
As2 K1 Cu 55.87(9) 1_455 2_666 ? 
As1 K1 Cu 142.82(15) . 2_666 ? 
O2 K1 Cu 37.0(2) 2_556 2_666 ? 
Cu2 K1 Cu 148.07(17) . 2_666 ? 
Fe K1 Cu 0.0 2_666 2_666 ? 
Al K1 Cu 0.0 2_666 2_666 ? 
O4 K1 Cu1 29.6(3) 2_566 1_455 ? 
O8 K1 Cu1 59.4(3) . 1_455 ? 
O9 K1 Cu1 96.8(3) . 1_455 ? 
O4 K1 Cu1 118.6(3) 2_666 1_455 ? 
O1 K1 Cu1 77.5(3) . 1_455 ? 
O2 K1 Cu1 76.9(3) . 1_455 ? 
O5 K1 Cu1 31.0(2) . 1_455 ? 
O6 K1 Cu1 129.6(3) . 1_455 ? 
Cu1 K1 Cu1 89.39(13) . 1_455 ? 
As2 K1 Cu1 118.75(14) . 1_455 ? 
As2 K1 Cu1 53.87(9) 1_455 1_455 ? 
As1 K1 Cu1 50.62(8) . 1_455 ? 
O2 K1 Cu1 114.3(2) 2_556 1_455 ? 
Cu2 K1 Cu1 96.82(12) . 1_455 ? 
Fe K1 Cu1 107.92(13) 2_666 1_455 ? 
Al K1 Cu1 107.92(13) 2_666 1_455 ? 
Cu K1 Cu1 107.92(13) 2_666 1_455 ? 
O4 K1 Ca1 90.2(3) 2_566 1_556 ? 
O8 K1 Ca1 56.3(3) . 1_556 ? 
O9 K1 Ca1 37.4(2) . 1_556 ? 
O4 K1 Ca1 85.6(3) 2_666 1_556 ? 
O1 K1 Ca1 130.6(3) . 1_556 ? 
O2 K1 Ca1 66.9(3) . 1_556 ? 
O5 K1 Ca1 36.1(2) . 1_556 ? 
O6 K1 Ca1 138.9(3) . 1_556 ? 
Cu1 K1 Ca1 53.77(8) . 1_556 ? 
As2 K1 Ca1 110.46(13) . 1_556 ? 
As2 K1 Ca1 114.46(14) 1_455 1_556 ? 
As1 K1 Ca1 49.20(7) . 1_556 ? 
O2 K1 Ca1 165.7(3) 2_556 1_556 ? 
Cu2 K1 Ca1 55.70(8) . 1_556 ? 
Fe K1 Ca1 155.47(15) 2_666 1_556 ? 
Al K1 Ca1 155.47(15) 2_666 1_556 ? 
Cu K1 Ca1 155.47(15) 2_666 1_556 ? 
Cu1 K1 Ca1 61.15(9) 1_455 1_556 ? 
O4 K1 Na1 90.2(3) 2_566 1_556 ? 
O8 K1 Na1 56.3(3) . 1_556 ? 
O9 K1 Na1 37.4(2) . 1_556 ? 
O4 K1 Na1 85.6(3) 2_666 1_556 ? 
O1 K1 Na1 130.6(3) . 1_556 ? 
O2 K1 Na1 66.9(3) . 1_556 ? 
O5 K1 Na1 36.1(2) . 1_556 ? 
O6 K1 Na1 138.9(3) . 1_556 ? 
Cu1 K1 Na1 53.77(8) . 1_556 ? 
As2 K1 Na1 110.46(13) . 1_556 ? 
As2 K1 Na1 114.46(14) 1_455 1_556 ? 
As1 K1 Na1 49.20(7) . 1_556 ? 
O2 K1 Na1 165.7(3) 2_556 1_556 ? 
Cu2 K1 Na1 55.70(8) . 1_556 ? 
Fe K1 Na1 155.47(15) 2_666 1_556 ? 
Al K1 Na1 155.47(15) 2_666 1_556 ? 
Cu K1 Na1 155.47(15) 2_666 1_556 ? 
Cu1 K1 Na1 61.15(9) 1_455 1_556 ? 
Ca1 K1 Na1 0.0 1_556 1_556 ? 
O5 Na1 O5 180.0(7) 2_666 1_554 ? 
O5 Na1 O9 87.8(5) 2_666 2_666 ? 
O5 Na1 O9 92.2(5) 1_554 2_666 ? 
O5 Na1 O9 92.2(5) 2_666 1_554 ? 
O5 Na1 O9 87.8(5) 1_554 1_554 ? 
O9 Na1 O9 180.0 2_666 1_554 ? 
O5 Na1 O3 62.6(4) 2_666 2_665 ? 
O5 Na1 O3 117.4(4) 1_554 2_665 ? 
O9 Na1 O3 81.9(4) 2_666 2_665 ? 
O9 Na1 O3 98.1(4) 1_554 2_665 ? 
O5 Na1 O3 117.4(4) 2_666 . ? 
O5 Na1 O3 62.6(4) 1_554 . ? 
O9 Na1 O3 98.1(4) 2_666 . ? 
O9 Na1 O3 81.9(4) 1_554 . ? 
O3 Na1 O3 180.000(1) 2_665 . ? 
O5 Na1 As1 31.2(3) 2_666 2_666 ? 
O5 Na1 As1 148.8(3) 1_554 2_666 ? 
O9 Na1 As1 76.4(3) 2_666 2_666 ? 
O9 Na1 As1 103.6(3) 1_554 2_666 ? 
O3 Na1 As1 33.0(3) 2_665 2_666 ? 
O3 Na1 As1 147.0(3) . 2_666 ? 
O5 Na1 As1 148.8(3) 2_666 1_554 ? 
O5 Na1 As1 31.2(3) 1_554 1_554 ? 
O9 Na1 As1 103.6(3) 2_666 1_554 ? 
O9 Na1 As1 76.4(3) 1_554 1_554 ? 
O3 Na1 As1 147.0(3) 2_665 1_554 ? 
O3 Na1 As1 33.0(3) . 1_554 ? 
As1 Na1 As1 180.0 2_666 1_554 ? 
O5 Na1 O8 113.5(4) 2_666 1_554 ? 
O5 Na1 O8 66.5(4) 1_554 1_554 ? 
O9 Na1 O8 99.1(4) 2_666 1_554 ? 
O9 Na1 O8 80.9(4) 1_554 1_554 ? 
O3 Na1 O8 53.5(3) 2_665 1_554 ? 
O3 Na1 O8 126.5(3) . 1_554 ? 
As1 Na1 O8 86.4(2) 2_666 1_554 ? 
As1 Na1 O8 93.6(2) 1_554 1_554 ? 
O5 Na1 O8 66.5(4) 2_666 2_666 ? 
O5 Na1 O8 113.5(4) 1_554 2_666 ? 
O9 Na1 O8 80.9(4) 2_666 2_666 ? 
O9 Na1 O8 99.1(4) 1_554 2_666 ? 
O3 Na1 O8 126.5(3) 2_665 2_666 ? 
O3 Na1 O8 53.5(3) . 2_666 ? 
As1 Na1 O8 93.6(2) 2_666 2_666 ? 
As1 Na1 O8 86.4(2) 1_554 2_666 ? 
O8 Na1 O8 180.000(1) 1_554 2_666 ? 
O5 Na1 Cu1 82.8(3) 2_666 1_554 ? 
O5 Na1 Cu1 97.2(3) 1_554 1_554 ? 
O9 Na1 Cu1 114.1(3) 2_666 1_554 ? 
O9 Na1 Cu1 65.9(3) 1_554 1_554 ? 
O3 Na1 Cu1 36.9(3) 2_665 1_554 ? 
O3 Na1 Cu1 143.1(3) . 1_554 ? 
As1 Na1 Cu1 62.92(5) 2_666 1_554 ? 
As1 Na1 Cu1 117.08(5) 1_554 1_554 ? 
O8 Na1 Cu1 34.4(2) 1_554 1_554 ? 
O8 Na1 Cu1 145.6(2) 2_666 1_554 ? 
O5 Na1 Cu1 97.2(3) 2_666 2_666 ? 
O5 Na1 Cu1 82.8(3) 1_554 2_666 ? 
O9 Na1 Cu1 65.9(3) 2_666 2_666 ? 
O9 Na1 Cu1 114.1(3) 1_554 2_666 ? 
O3 Na1 Cu1 143.1(3) 2_665 2_666 ? 
O3 Na1 Cu1 36.9(3) . 2_666 ? 
As1 Na1 Cu1 117.08(5) 2_666 2_666 ? 
As1 Na1 Cu1 62.92(5) 1_554 2_666 ? 
O8 Na1 Cu1 145.6(2) 1_554 2_666 ? 
O8 Na1 Cu1 34.4(2) 2_666 2_666 ? 
Cu1 Na1 Cu1 180.0 1_554 2_666 ? 
O5 Na1 As1 65.9(4) 2_666 1_654 ? 
O5 Na1 As1 114.1(4) 1_554 1_654 ? 
O9 Na1 As1 152.1(3) 2_666 1_654 ? 
O9 Na1 As1 27.9(3) 1_554 1_654 ? 
O3 Na1 As1 78.0(3) 2_665 1_654 ? 
O3 Na1 As1 102.0(3) . 1_654 ? 
As1 Na1 As1 76.20(5) 2_666 1_654 ? 
As1 Na1 As1 103.80(5) 1_554 1_654 ? 
O8 Na1 As1 84.2(2) 1_554 1_654 ? 
O8 Na1 As1 95.8(2) 2_666 1_654 ? 
Cu1 Na1 As1 56.10(5) 1_554 1_654 ? 
Cu1 Na1 As1 123.90(5) 2_666 1_654 ? 
O5 Na1 As1 114.1(4) 2_666 2_566 ? 
O5 Na1 As1 65.9(4) 1_554 2_566 ? 
O9 Na1 As1 27.9(3) 2_666 2_566 ? 
O9 Na1 As1 152.1(3) 1_554 2_566 ? 
O3 Na1 As1 102.0(3) 2_665 2_566 ? 
O3 Na1 As1 78.0(3) . 2_566 ? 
As1 Na1 As1 103.80(5) 2_666 2_566 ? 
As1 Na1 As1 76.20(5) 1_554 2_566 ? 
O8 Na1 As1 95.8(2) 1_554 2_566 ? 
O8 Na1 As1 84.2(2) 2_666 2_566 ? 
Cu1 Na1 As1 123.90(5) 1_554 2_566 ? 
Cu1 Na1 As1 56.10(5) 2_666 2_566 ? 
As1 Na1 As1 180.00(7) 1_654 2_566 ? 
O5 Na1 Cu2 76.3(3) 2_666 2_666 ? 
O5 Na1 Cu2 103.7(3) 1_554 2_666 ? 
O9 Na1 Cu2 32.4(3) 2_666 2_666 ? 
O9 Na1 Cu2 147.6(3) 1_554 2_666 ? 
O3 Na1 Cu2 49.6(3) 2_665 2_666 ? 
O3 Na1 Cu2 130.4(3) . 2_666 ? 
As1 Na1 Cu2 52.57(5) 2_666 2_666 ? 
As1 Na1 Cu2 127.43(5) 1_554 2_666 ? 
O8 Na1 Cu2 76.4(2) 1_554 2_666 ? 
O8 Na1 Cu2 103.6(2) 2_666 2_666 ? 
Cu1 Na1 Cu2 82.41(6) 1_554 2_666 ? 
Cu1 Na1 Cu2 97.59(6) 2_666 2_666 ? 
As1 Na1 Cu2 125.58(5) 1_654 2_666 ? 
As1 Na1 Cu2 54.42(5) 2_566 2_666 ? 
O5 Na1 Cu2 103.7(3) 2_666 1_554 ? 
O5 Na1 Cu2 76.3(3) 1_554 1_554 ? 
O9 Na1 Cu2 147.6(3) 2_666 1_554 ? 
O9 Na1 Cu2 32.4(3) 1_554 1_554 ? 
O3 Na1 Cu2 130.4(3) 2_665 1_554 ? 
O3 Na1 Cu2 49.6(3) . 1_554 ? 
As1 Na1 Cu2 127.43(5) 2_666 1_554 ? 
As1 Na1 Cu2 52.57(5) 1_554 1_554 ? 
O8 Na1 Cu2 103.6(2) 1_554 1_554 ? 
O8 Na1 Cu2 76.4(2) 2_666 1_554 ? 
Cu1 Na1 Cu2 97.59(6) 1_554 1_554 ? 
Cu1 Na1 Cu2 82.41(6) 2_666 1_554 ? 
As1 Na1 Cu2 54.42(5) 1_654 1_554 ? 
As1 Na1 Cu2 125.58(5) 2_566 1_554 ? 
Cu2 Na1 Cu2 180.0 2_666 1_554 ? 
O5 Na1 O5 60.7(5) 2_666 1_654 ? 
O5 Na1 O5 119.3(5) 1_554 1_654 ? 
O9 Na1 O5 130.7(4) 2_666 1_654 ? 
O9 Na1 O5 49.3(4) 1_554 1_654 ? 
O3 Na1 O5 50.8(3) 2_665 1_654 ? 
O3 Na1 O5 129.2(3) . 1_654 ? 
As1 Na1 O5 56.7(2) 2_666 1_654 ? 
As1 Na1 O5 123.3(2) 1_554 1_654 ? 
O8 Na1 O5 66.1(3) 1_554 1_654 ? 
O8 Na1 O5 113.9(3) 2_666 1_654 ? 
Cu1 Na1 O5 32.73(19) 1_554 1_654 ? 
Cu1 Na1 O5 147.27(19) 2_666 1_654 ? 
As1 Na1 O5 27.5(2) 1_654 1_654 ? 
As1 Na1 O5 152.5(2) 2_566 1_654 ? 
Cu2 Na1 O5 99.7(2) 2_666 1_654 ? 
Cu2 Na1 O5 80.3(2) 1_554 1_654 ? 
O5 Na1 O5 119.3(5) 2_666 2_566 ? 
O5 Na1 O5 60.7(5) 1_554 2_566 ? 
O9 Na1 O5 49.3(4) 2_666 2_566 ? 
O9 Na1 O5 130.7(4) 1_554 2_566 ? 
O3 Na1 O5 129.2(3) 2_665 2_566 ? 
O3 Na1 O5 50.8(3) . 2_566 ? 
As1 Na1 O5 123.3(2) 2_666 2_566 ? 
As1 Na1 O5 56.7(2) 1_554 2_566 ? 
O8 Na1 O5 113.9(3) 1_554 2_566 ? 
O8 Na1 O5 66.1(3) 2_666 2_566 ? 
Cu1 Na1 O5 147.27(19) 1_554 2_566 ? 
Cu1 Na1 O5 32.73(19) 2_666 2_566 ? 
As1 Na1 O5 152.5(2) 1_654 2_566 ? 
As1 Na1 O5 27.5(2) 2_566 2_566 ? 
Cu2 Na1 O5 80.3(2) 2_666 2_566 ? 
Cu2 Na1 O5 99.7(2) 1_554 2_566 ? 
O5 Na1 O5 180.00(16) 1_654 2_566 ? 
O5 Na1 O2 45.1(4) 2_666 2_666 ? 
O5 Na1 O2 134.9(4) 1_554 2_666 ? 
O9 Na1 O2 50.7(4) 2_666 2_666 ? 
O9 Na1 O2 129.3(4) 1_554 2_666 ? 
O3 Na1 O2 43.8(3) 2_665 2_666 ? 
O3 Na1 O2 136.2(3) . 2_666 ? 
As1 Na1 O2 25.7(2) 2_666 2_666 ? 
As1 Na1 O2 154.3(2) 1_554 2_666 ? 
O8 Na1 O2 92.1(3) 1_554 2_666 ? 
O8 Na1 O2 87.9(3) 2_666 2_666 ? 
Cu1 Na1 O2 80.3(2) 1_554 2_666 ? 
Cu1 Na1 O2 99.7(2) 2_666 2_666 ? 
As1 Na1 O2 101.7(2) 1_654 2_666 ? 
As1 Na1 O2 78.3(2) 2_566 2_666 ? 
Cu2 Na1 O2 31.2(2) 2_666 2_666 ? 
Cu2 Na1 O2 148.8(2) 1_554 2_666 ? 
O5 Na1 O2 81.8(3) 1_654 2_666 ? 
O5 Na1 O2 98.2(3) 2_566 2_666 ? 
O5 Na1 O2 134.9(4) 2_666 1_554 ? 
O5 Na1 O2 45.1(4) 1_554 1_554 ? 
O9 Na1 O2 129.3(4) 2_666 1_554 ? 
O9 Na1 O2 50.7(4) 1_554 1_554 ? 
O3 Na1 O2 136.2(3) 2_665 1_554 ? 
O3 Na1 O2 43.8(3) . 1_554 ? 
As1 Na1 O2 154.3(2) 2_666 1_554 ? 
As1 Na1 O2 25.7(2) 1_554 1_554 ? 
O8 Na1 O2 87.9(3) 1_554 1_554 ? 
O8 Na1 O2 92.1(3) 2_666 1_554 ? 
Cu1 Na1 O2 99.7(2) 1_554 1_554 ? 
Cu1 Na1 O2 80.3(2) 2_666 1_554 ? 
As1 Na1 O2 78.3(2) 1_654 1_554 ? 
As1 Na1 O2 101.7(2) 2_566 1_554 ? 
Cu2 Na1 O2 148.8(2) 2_666 1_554 ? 
Cu2 Na1 O2 31.2(2) 1_554 1_554 ? 
O5 Na1 O2 98.2(3) 1_654 1_554 ? 
O5 Na1 O2 81.8(3) 2_566 1_554 ? 
O2 Na1 O2 180.0 2_666 1_554 ? 
O5 As1 O9 108.3(6) . 1_455 ? 
O5 As1 O2 110.0(7) . . ? 
O9 As1 O2 112.5(7) 1_455 . ? 
O5 As1 O3 105.3(7) . 1_556 ? 
O9 As1 O3 117.9(6) 1_455 1_556 ? 
O2 As1 O3 102.4(6) . 1_556 ? 
O5 As1 Cu2 103.9(4) . . ? 
O9 As1 Cu2 144.6(4) 1_455 . ? 
O2 As1 Cu2 40.4(5) . . ? 
O3 As1 Cu2 65.4(4) 1_556 . ? 
O5 As1 Ca1 45.7(4) . 1_556 ? 
O9 As1 Ca1 143.8(4) 1_455 1_556 ? 
O2 As1 Ca1 101.7(5) . 1_556 ? 
O3 As1 Ca1 63.1(5) 1_556 1_556 ? 
Cu2 As1 Ca1 71.09(6) . 1_556 ? 
O5 As1 Na1 45.7(4) . 1_556 ? 
O9 As1 Na1 143.8(4) 1_455 1_556 ? 
O2 As1 Na1 101.7(5) . 1_556 ? 
O3 As1 Na1 63.1(5) 1_556 1_556 ? 
Cu2 As1 Na1 71.09(6) . 1_556 ? 
Ca1 As1 Na1 0.0 1_556 1_556 ? 
O5 As1 Cu1 32.3(4) . 1_455 ? 
O9 As1 Cu1 76.7(4) 1_455 1_455 ? 
O2 As1 Cu1 118.4(5) . 1_455 ? 
O3 As1 Cu1 127.5(5) 1_556 1_455 ? 
Cu2 As1 Cu1 131.82(9) . 1_455 ? 
Ca1 As1 Cu1 76.80(6) 1_556 1_455 ? 
Na1 As1 Cu1 76.80(6) 1_556 1_455 ? 
O5 As1 Cu2 142.3(4) . 1_455 ? 
O9 As1 Cu2 34.0(4) 1_455 1_455 ? 
O2 As1 Cu2 92.0(5) . 1_455 ? 
O3 As1 Cu2 99.0(5) 1_556 1_455 ? 
Cu2 As1 Cu2 112.44(9) . 1_455 ? 
Ca1 As1 Cu2 159.24(8) 1_556 1_455 ? 
Na1 As1 Cu2 159.24(8) 1_556 1_455 ? 
Cu1 As1 Cu2 110.35(8) 1_455 1_455 ? 
O5 As1 Cu 141.2(4) . 2_667 ? 
O9 As1 Cu 99.8(4) 1_455 2_667 ? 
O2 As1 Cu 81.9(5) . 2_667 ? 
O3 As1 Cu 36.4(5) 1_556 2_667 ? 
Cu2 As1 Cu 60.97(8) . 2_667 ? 
Ca1 As1 Cu 96.44(7) 1_556 2_667 ? 
Na1 As1 Cu 96.44(7) 1_556 2_667 ? 
Cu1 As1 Cu 159.34(10) 1_455 2_667 ? 
Cu2 As1 Cu 69.89(8) 1_455 2_667 ? 
O5 As1 Cu 151.6(5) . 1_445 ? 
O9 As1 Cu 87.2(4) 1_455 1_445 ? 
O2 As1 Cu 41.6(5) . 1_445 ? 
O3 As1 Cu 86.8(5) 1_556 1_445 ? 
Cu2 As1 Cu 57.45(7) . 1_445 ? 
Ca1 As1 Cu 127.84(8) 1_556 1_445 ? 
Na1 As1 Cu 127.84(8) 1_556 1_445 ? 
Cu1 As1 Cu 145.66(9) 1_455 1_445 ? 
Cu2 As1 Cu 56.36(7) 1_455 1_445 ? 
Cu As1 Cu 52.65(10) 2_667 1_445 ? 
O5 As1 Ca1 83.4(5) . 1_456 ? 
O9 As1 Ca1 41.1(4) 1_455 1_456 ? 
O2 As1 Ca1 153.5(5) . 1_456 ? 
O3 As1 Ca1 95.5(4) 1_556 1_456 ? 
Cu2 As1 Ca1 160.63(8) . 1_456 ? 
Ca1 As1 Ca1 103.80(5) 1_556 1_456 ? 
Na1 As1 Ca1 103.80(5) 1_556 1_456 ? 
Cu1 As1 Ca1 61.65(6) 1_455 1_456 ? 
Cu2 As1 Ca1 65.74(6) 1_455 1_456 ? 
Cu As1 Ca1 102.14(7) 2_667 1_456 ? 
Cu As1 Ca1 121.61(7) 1_445 1_456 ? 
O4 As2 O8 115.8(7) 2_666 2_666 ? 
O4 As2 O6 105.9(6) 2_666 . ? 
O8 As2 O6 110.2(6) 2_666 . ? 
O4 As2 O1 103.0(7) 2_666 1_655 ? 
O8 As2 O1 110.3(6) 2_666 1_655 ? 
O6 As2 O1 111.4(7) . 1_655 ? 
O4 As2 Cu 121.3(5) 2_666 2_666 ? 
O8 As2 Cu 83.2(4) 2_666 2_666 ? 
O6 As2 Cu 27.0(5) . 2_666 ? 
O1 As2 Cu 122.3(5) 1_655 2_666 ? 
O4 As2 Cu1 117.1(5) 2_666 2_666 ? 
O8 As2 Cu1 28.0(4) 2_666 2_666 ? 
O6 As2 Cu1 83.8(5) . 2_666 ? 
O1 As2 Cu1 131.5(4) 1_655 2_666 ? 
Cu As2 Cu1 57.60(7) 2_666 2_666 ? 
O4 As2 Cu1 25.9(5) 2_666 . ? 
O8 As2 Cu1 90.1(5) 2_666 . ? 
O6 As2 Cu1 121.4(4) . . ? 
O1 As2 Cu1 111.3(5) 1_655 . ? 
Cu As2 Cu1 124.96(9) 2_666 . ? 
Cu1 As2 Cu1 96.28(8) 2_666 . ? 
O4 As2 Cu 114.7(5) 2_666 2_766 ? 
O8 As2 Cu 116.8(5) 2_666 2_766 ? 
O6 As2 Cu 89.4(4) . 2_766 ? 
O1 As2 Cu 22.5(5) 1_655 2_766 ? 
Cu As2 Cu 100.57(9) 2_666 2_766 ? 
Cu1 As2 Cu 127.65(9) 2_666 2_766 ? 
Cu1 As2 Cu 130.11(9) . 2_766 ? 
O4 As2 Cu1 110.9(5) 2_666 2_766 ? 
O8 As2 Cu1 73.5(5) 2_666 2_766 ? 
O6 As2 Cu1 136.5(4) . 2_766 ? 
O1 As2 Cu1 38.4(4) 1_655 2_766 ? 
Cu As2 Cu1 127.78(9) 2_666 2_766 ? 
Cu1 As2 Cu1 98.93(8) 2_666 2_766 ? 
Cu1 As2 Cu1 101.57(7) . 2_766 ? 
Cu As2 Cu1 54.67(7) 2_766 2_766 ? 
O4 As2 K1 54.7(5) 2_666 . ? 
O8 As2 K1 103.2(5) 2_666 . ? 
O6 As2 K1 60.6(4) . . ? 
O1 As2 K1 145.8(4) 1_655 . ? 
Cu As2 K1 67.28(10) 2_666 . ? 
Cu1 As2 K1 82.31(10) 2_666 . ? 
Cu1 As2 K1 61.34(10) . . ? 
Cu As2 K1 136.75(12) 2_766 . ? 
Cu1 As2 K1 162.82(12) 2_766 . ? 
O4 As2 K1 49.3(5) 2_666 1_655 ? 
O8 As2 K1 140.8(4) 2_666 1_655 ? 
O6 As2 K1 109.0(5) . 1_655 ? 
O1 As2 K1 55.6(4) 1_655 1_655 ? 
Cu As2 K1 135.92(11) 2_666 1_655 ? 
Cu1 As2 K1 162.80(12) 2_666 1_655 ? 
Cu1 As2 K1 67.41(10) . 1_655 ? 
Cu As2 K1 65.58(10) 2_766 1_655 ? 
Cu1 As2 K1 79.93(10) 2_766 1_655 ? 
K1 As2 K1 93.80(12) . 1_655 ? 
O4 As2 Cu2 118.2(5) 2_666 2_656 ? 
O8 As2 Cu2 122.9(4) 2_666 2_656 ? 
O6 As2 Cu2 37.3(4) . 2_656 ? 
O1 As2 Cu2 74.2(5) 1_655 2_656 ? 
Cu As2 Cu2 53.64(7) 2_666 2_656 ? 
Cu1 As2 Cu2 106.44(8) 2_666 2_656 ? 
Cu1 As2 Cu2 143.39(8) . 2_656 ? 
Cu As2 Cu2 52.05(7) 2_766 2_656 ? 
Cu1 As2 Cu2 102.76(7) 2_766 2_656 ? 
K1 As2 Cu2 93.21(11) . 2_656 ? 
K1 As2 Cu2 90.47(11) 1_655 2_656 ? 
O4 Cu1 O8 91.5(6) 2_666 . ? 
O4 Cu1 O5 87.6(6) 2_666 1_655 ? 
O8 Cu1 O5 146.1(5) . 1_655 ? 
O4 Cu1 O3 176.9(6) 2_666 2_666 ? 
O8 Cu1 O3 88.7(5) . 2_666 ? 
O5 Cu1 O3 90.5(6) 1_655 2_666 ? 
O4 Cu1 O1 104.9(5) 2_666 2_666 ? 
O8 Cu1 O1 98.4(5) . 2_666 ? 
O5 Cu1 O1 114.5(5) 1_655 2_666 ? 
O3 Cu1 O1 78.2(5) 2_666 2_666 ? 
O4 Cu1 Cu 139.2(4) 2_666 . ? 
O8 Cu1 Cu 82.2(4) . . ? 
O5 Cu1 Cu 119.1(4) 1_655 . ? 
O3 Cu1 Cu 43.8(4) 2_666 . ? 
O1 Cu1 Cu 37.9(3) 2_666 . ? 
O4 Cu1 As1 81.6(4) 2_666 1_655 ? 
O8 Cu1 As1 119.7(4) . 1_655 ? 
O5 Cu1 As1 26.9(4) 1_655 1_655 ? 
O3 Cu1 As1 95.6(4) 2_666 1_655 ? 
O1 Cu1 As1 141.4(3) 2_666 1_655 ? 
Cu Cu1 As1 135.99(10) . 1_655 ? 
O4 Cu1 O9 82.8(4) 2_666 . ? 
O8 Cu1 O9 89.1(4) . . ? 
O5 Cu1 O9 57.2(4) 1_655 . ? 
O3 Cu1 O9 94.1(5) 2_666 . ? 
O1 Cu1 O9 169.0(4) 2_666 . ? 
Cu Cu1 O9 136.9(2) . . ? 
As1 Cu1 O9 30.6(2) 1_655 . ? 
O4 Cu1 As2 101.8(4) 2_666 2_666 ? 
O8 Cu1 As2 23.6(4) . 2_666 ? 
O5 Cu1 As2 164.5(4) 1_655 2_666 ? 
O3 Cu1 As2 79.5(4) 2_666 2_666 ? 
O1 Cu1 As2 75.3(3) 2_666 2_666 ? 
Cu Cu1 As2 60.62(8) . 2_666 ? 
As1 Cu1 As2 141.70(9) 1_655 2_666 ? 
O9 Cu1 As2 111.3(2) . 2_666 ? 
O4 Cu1 As2 22.0(4) 2_666 . ? 
O8 Cu1 As2 79.6(4) . . ? 
O5 Cu1 As2 107.8(4) 1_655 . ? 
O3 Cu1 As2 160.7(4) 2_666 . ? 
O1 Cu1 As2 88.3(4) 2_666 . ? 
Cu Cu1 As2 118.50(10) . . ? 
As1 Cu1 As2 103.56(8) 1_655 . ? 
O9 Cu1 As2 101.0(2) . . ? 
As2 Cu1 As2 83.72(8) 2_666 . ? 
O4 Cu1 Ca1 120.6(4) 2_666 1_556 ? 
O8 Cu1 Ca1 71.3(4) . 1_556 ? 
O5 Cu1 Ca1 80.1(4) 1_655 1_556 ? 
O3 Cu1 Ca1 56.6(4) 2_666 1_556 ? 
O1 Cu1 Ca1 133.2(4) 2_666 1_556 ? 
Cu Cu1 Ca1 95.50(8) . 1_556 ? 
As1 Cu1 Ca1 62.25(6) 1_655 1_556 ? 
O9 Cu1 Ca1 42.3(2) . 1_556 ? 
As2 Cu1 Ca1 84.50(7) 2_666 1_556 ? 
As2 Cu1 Ca1 131.35(8) . 1_556 ? 
O4 Cu1 Na1 120.6(4) 2_666 1_556 ? 
O8 Cu1 Na1 71.3(4) . 1_556 ? 
O5 Cu1 Na1 80.1(4) 1_655 1_556 ? 
O3 Cu1 Na1 56.6(4) 2_666 1_556 ? 
O1 Cu1 Na1 133.2(4) 2_666 1_556 ? 
Cu Cu1 Na1 95.50(8) . 1_556 ? 
As1 Cu1 Na1 62.25(6) 1_655 1_556 ? 
O9 Cu1 Na1 42.3(2) . 1_556 ? 
As2 Cu1 Na1 84.50(7) 2_666 1_556 ? 
As2 Cu1 Na1 131.35(8) . 1_556 ? 
Ca1 Cu1 Na1 0.0 1_556 1_556 ? 
O4 Cu1 O8 77.3(5) 2_666 1_655 ? 
O8 Cu1 O8 145.3(6) . 1_655 ? 
O5 Cu1 O8 67.1(4) 1_655 1_655 ? 
O3 Cu1 O8 104.2(4) 2_666 1_655 ? 
O1 Cu1 O8 54.6(4) 2_666 1_655 ? 
Cu Cu1 O8 85.3(2) . 1_655 ? 
As1 Cu1 O8 91.5(2) 1_655 1_655 ? 
O9 Cu1 O8 121.2(3) . 1_655 ? 
As2 Cu1 O8 126.7(2) 2_666 1_655 ? 
As2 Cu1 O8 78.3(2) . 1_655 ? 
Ca1 Cu1 O8 142.4(2) 1_556 1_655 ? 
Na1 Cu1 O8 142.4(2) 1_556 1_655 ? 
O4 Cu1 As1 155.4(4) 2_666 2_667 ? 
O8 Cu1 As1 107.7(4) . 2_667 ? 
O5 Cu1 As1 67.9(4) 1_655 2_667 ? 
O3 Cu1 As1 22.7(4) 2_666 2_667 ? 
O1 Cu1 As1 87.9(4) 2_666 2_667 ? 
Cu Cu1 As1 61.02(8) . 2_667 ? 
As1 Cu1 As1 75.52(7) 1_655 2_667 ? 
O9 Cu1 As1 82.2(2) . 2_667 ? 
As2 Cu1 As1 101.83(8) 2_666 2_667 ? 
As2 Cu1 As1 172.23(9) . 2_667 ? 
Ca1 Cu1 As1 55.29(5) 1_556 2_667 ? 
Na1 Cu1 As1 55.29(5) 1_556 2_667 ? 
O8 Cu1 As1 94.0(2) 1_655 2_667 ? 
O4 Cu1 As2 88.0(4) 2_666 2_766 ? 
O8 Cu1 As2 120.2(4) . 2_766 ? 
O5 Cu1 As2 93.7(4) 1_655 2_766 ? 
O3 Cu1 As2 94.6(4) 2_666 2_766 ? 
O1 Cu1 As2 26.8(3) 2_666 2_766 ? 
Cu Cu1 As2 61.96(8) . 2_766 ? 
As1 Cu1 As2 119.35(9) 1_655 2_766 ? 
O9 Cu1 As2 149.6(2) . 2_766 ? 
As2 Cu1 As2 98.93(8) 2_666 2_766 ? 
As2 Cu1 As2 78.43(7) . 2_766 ? 
Ca1 Cu1 As2 150.13(8) 1_556 2_766 ? 
Na1 Cu1 As2 150.13(8) 1_556 2_766 ? 
O8 Cu1 As2 28.5(2) 1_655 2_766 ? 
As1 Cu1 As2 95.21(8) 2_667 2_766 ? 
O4 Cu1 K1 55.8(4) 2_666 . ? 
O8 Cu1 K1 53.6(4) . . ? 
O5 Cu1 K1 99.7(4) 1_655 . ? 
O3 Cu1 K1 122.2(4) 2_666 . ? 
O1 Cu1 K1 140.6(4) 2_666 . ? 
Cu Cu1 K1 135.64(13) . . ? 
As1 Cu1 K1 74.67(10) 1_655 . ? 
O9 Cu1 K1 50.3(2) . . ? 
As2 Cu1 K1 76.18(10) 2_666 . ? 
As2 Cu1 K1 61.97(10) . . ? 
Ca1 Cu1 K1 69.38(9) 1_556 . ? 
Na1 Cu1 K1 69.38(9) 1_556 . ? 
O8 Cu1 K1 132.3(3) 1_655 . ? 
As1 Cu1 K1 124.40(11) 2_667 . ? 
As2 Cu1 K1 140.36(11) 2_766 . ? 
O4 Cu1 O6 120.0(4) 2_666 2_666 ? 
O8 Cu1 O6 51.3(4) . 2_666 ? 
O5 Cu1 O6 150.4(5) 1_655 2_666 ? 
O3 Cu1 O6 62.3(4) 2_666 2_666 ? 
O1 Cu1 O6 51.8(4) 2_666 2_666 ? 
Cu Cu1 O6 32.5(2) . 2_666 ? 
As1 Cu1 O6 154.0(2) 1_655 2_666 ? 
O9 Cu1 O6 131.1(3) . 2_666 ? 
As2 Cu1 O6 28.5(2) 2_666 2_666 ? 
As2 Cu1 O6 98.5(2) . 2_666 ? 
Ca1 Cu1 O6 92.8(2) 1_556 2_666 ? 
Na1 Cu1 O6 92.8(2) 1_556 2_666 ? 
O8 Cu1 O6 106.4(3) 1_655 2_666 ? 
As1 Cu1 O6 84.4(2) 2_667 2_666 ? 
As2 Cu1 O6 78.3(2) 2_766 2_666 ? 
K1 Cu1 O6 104.6(2) . 2_666 ? 
O4 Cu1 O8 48.7(4) 2_666 2_666 ? 
O8 Cu1 O8 63.8(5) . 2_666 ? 
O5 Cu1 O8 133.2(5) 1_655 2_666 ? 
O3 Cu1 O8 133.8(5) 2_666 2_666 ? 
O1 Cu1 O8 70.8(4) 2_666 2_666 ? 
Cu Cu1 O8 93.7(2) . 2_666 ? 
As1 Cu1 O8 129.8(2) 1_655 2_666 ? 
O9 Cu1 O8 119.9(3) . 2_666 ? 
As2 Cu1 O8 60.3(2) 2_666 2_666 ? 
As2 Cu1 O8 26.8(2) . 2_666 ? 
Ca1 Cu1 O8 132.3(2) 1_556 2_666 ? 
Na1 Cu1 O8 132.3(2) 1_556 2_666 ? 
O8 Cu1 O8 84.9(3) 1_655 2_666 ? 
As1 Cu1 O8 154.6(2) 2_667 2_666 ? 
As2 Cu1 O8 72.1(2) 2_766 2_666 ? 
K1 Cu1 O8 71.6(2) . 2_666 ? 
O6 Cu1 O8 71.7(3) 2_666 2_666 ? 
O7 Cu2 O7 87.0(5) 2_657 . ? 
O7 Cu2 O9 93.5(5) 2_657 . ? 
O7 Cu2 O9 164.4(5) . . ? 
O7 Cu2 O2 169.6(5) 2_657 . ? 
O7 Cu2 O2 85.1(5) . . ? 
O9 Cu2 O2 95.9(5) . . ? 
O7 Cu2 O6 75.4(5) 2_657 2_656 ? 
O7 Cu2 O6 96.3(5) . 2_656 ? 
O9 Cu2 O6 98.9(4) . 2_656 ? 
O2 Cu2 O6 98.7(5) . 2_656 ? 
O7 Cu2 O3 118.5(4) 2_657 1_556 ? 
O7 Cu2 O3 76.1(5) . 1_556 ? 
O9 Cu2 O3 90.1(5) . 1_556 ? 
O2 Cu2 O3 66.0(5) . 1_556 ? 
O6 Cu2 O3 163.2(4) 2_656 1_556 ? 
O7 Cu2 Cu2 43.8(4) 2_657 2_657 ? 
O7 Cu2 Cu2 43.2(4) . 2_657 ? 
O9 Cu2 Cu2 135.2(4) . 2_657 ? 
O2 Cu2 Cu2 127.9(4) . 2_657 ? 
O6 Cu2 Cu2 84.5(3) 2_656 2_657 ? 
O3 Cu2 Cu2 99.2(3) 1_556 2_657 ? 
O7 Cu2 As1 152.8(4) 2_657 . ? 
O7 Cu2 As1 87.2(4) . . ? 
O9 Cu2 As1 85.2(4) . . ? 
O2 Cu2 As1 33.4(4) . . ? 
O6 Cu2 As1 131.7(3) 2_656 . ? 
O3 Cu2 As1 34.5(3) 1_556 . ? 
Cu2 Cu2 As1 125.14(13) 2_657 . ? 
O7 Cu2 Fe 120.1(4) 2_657 1_445 ? 
O7 Cu2 Fe 38.2(3) . 1_445 ? 
O9 Cu2 Fe 146.1(4) . 1_445 ? 
O2 Cu2 Fe 50.2(4) . 1_445 ? 
O6 Cu2 Fe 86.7(3) 2_656 1_445 ? 
O3 Cu2 Fe 78.0(3) 1_556 1_445 ? 
Cu2 Cu2 Fe 78.40(10) 2_657 1_445 ? 
As1 Cu2 Fe 66.98(8) . 1_445 ? 
O7 Cu2 Al 120.1(4) 2_657 1_445 ? 
O7 Cu2 Al 38.2(3) . 1_445 ? 
O9 Cu2 Al 146.1(4) . 1_445 ? 
O2 Cu2 Al 50.2(4) . 1_445 ? 
O6 Cu2 Al 86.7(3) 2_656 1_445 ? 
O3 Cu2 Al 78.0(3) 1_556 1_445 ? 
Cu2 Cu2 Al 78.40(10) 2_657 1_445 ? 
As1 Cu2 Al 66.98(8) . 1_445 ? 
Fe Cu2 Al 0.00(10) 1_445 1_445 ? 
O7 Cu2 Cu 120.1(4) 2_657 1_445 ? 
O7 Cu2 Cu 38.2(3) . 1_445 ? 
O9 Cu2 Cu 146.1(4) . 1_445 ? 
O2 Cu2 Cu 50.2(4) . 1_445 ? 
O6 Cu2 Cu 86.7(3) 2_656 1_445 ? 
O3 Cu2 Cu 78.0(3) 1_556 1_445 ? 
Cu2 Cu2 Cu 78.40(10) 2_657 1_445 ? 
As1 Cu2 Cu 66.98(8) . 1_445 ? 
Fe Cu2 Cu 0.00(10) 1_445 1_445 ? 
Al Cu2 Cu 0.00(10) 1_445 1_445 ? 
O7 Cu2 Fe 38.7(4) 2_657 1_545 ? 
O7 Cu2 Fe 100.3(4) . 1_545 ? 
O9 Cu2 Fe 89.6(4) . 1_545 ? 
O2 Cu2 Fe 136.8(4) . 1_545 ? 
O6 Cu2 Fe 38.2(3) 2_656 1_545 ? 
O3 Cu2 Fe 157.1(3) 1_556 1_545 ? 
Cu2 Cu2 Fe 65.75(10) 2_657 1_545 ? 
As1 Cu2 Fe 167.63(11) . 1_545 ? 
Fe Cu2 Fe 113.39(11) 1_445 1_545 ? 
Al Cu2 Fe 113.39(11) 1_445 1_545 ? 
Cu Cu2 Fe 113.39(11) 1_445 1_545 ? 
O7 Cu2 Al 38.7(4) 2_657 1_545 ? 
O7 Cu2 Al 100.3(4) . 1_545 ? 
O9 Cu2 Al 89.6(4) . 1_545 ? 
O2 Cu2 Al 136.8(4) . 1_545 ? 
O6 Cu2 Al 38.2(3) 2_656 1_545 ? 
O3 Cu2 Al 157.1(3) 1_556 1_545 ? 
Cu2 Cu2 Al 65.75(10) 2_657 1_545 ? 
As1 Cu2 Al 167.63(11) . 1_545 ? 
Fe Cu2 Al 113.39(11) 1_445 1_545 ? 
Al Cu2 Al 113.39(11) 1_445 1_545 ? 
Cu Cu2 Al 113.39(11) 1_445 1_545 ? 
Fe Cu2 Al 0.00(18) 1_545 1_545 ? 
O7 Cu2 Cu 38.7(4) 2_657 1_545 ? 
O7 Cu2 Cu 100.3(4) . 1_545 ? 
O9 Cu2 Cu 89.6(4) . 1_545 ? 
O2 Cu2 Cu 136.8(4) . 1_545 ? 
O6 Cu2 Cu 38.2(3) 2_656 1_545 ? 
O3 Cu2 Cu 157.1(3) 1_556 1_545 ? 
Cu2 Cu2 Cu 65.75(10) 2_657 1_545 ? 
As1 Cu2 Cu 167.63(11) . 1_545 ? 
Fe Cu2 Cu 113.39(11) 1_445 1_545 ? 
Al Cu2 Cu 113.39(11) 1_445 1_545 ? 
Cu Cu2 Cu 113.39(11) 1_445 1_545 ? 
Fe Cu2 Cu 0.00(18) 1_545 1_545 ? 
Al Cu2 Cu 0.00(18) 1_545 1_545 ? 
O7 Cu2 As1 66.3(4) 2_657 1_655 ? 
O7 Cu2 As1 152.0(4) . 1_655 ? 
O9 Cu2 As1 28.0(4) . 1_655 ? 
O2 Cu2 As1 122.4(4) . 1_655 ? 
O6 Cu2 As1 85.4(3) 2_656 1_655 ? 
O3 Cu2 As1 108.4(3) 1_556 1_655 ? 
Cu2 Cu2 As1 109.69(12) 2_657 1_655 ? 
As1 Cu2 As1 112.44(9) . 1_655 ? 
Fe Cu2 As1 168.05(11) 1_445 1_655 ? 
Al Cu2 As1 168.05(11) 1_445 1_655 ? 
Cu Cu2 As1 168.05(11) 1_445 1_655 ? 
Fe Cu2 As1 64.42(8) 1_545 1_655 ? 
Al Cu2 As1 64.42(8) 1_545 1_655 ? 
Cu Cu2 As1 64.42(8) 1_545 1_655 ? 
O7 Cu2 Fe 96.3(4) 2_657 2_667 ? 
O7 Cu2 Fe 35.5(4) . 2_667 ? 
O9 Cu2 Fe 129.2(4) . 2_667 ? 
O2 Cu2 Fe 81.1(4) . 2_667 ? 
O6 Cu2 Fe 131.8(3) 2_656 2_667 ? 
O3 Cu2 Fe 42.3(3) 1_556 2_667 ? 
Cu2 Cu2 Fe 60.71(10) 2_657 2_667 ? 
As1 Cu2 Fe 64.74(8) . 2_667 ? 
Fe Cu2 Fe 56.15(11) 1_445 2_667 ? 
Al Cu2 Fe 56.15(11) 1_445 2_667 ? 
Cu Cu2 Fe 56.15(11) 1_445 2_667 ? 
Fe Cu2 Fe 126.46(9) 1_545 2_667 ? 
Al Cu2 Fe 126.46(9) 1_545 2_667 ? 
Cu Cu2 Fe 126.46(9) 1_545 2_667 ? 
As1 Cu2 Fe 135.25(10) 1_655 2_667 ? 
O7 Cu2 Al 96.3(4) 2_657 2_667 ? 
O7 Cu2 Al 35.5(4) . 2_667 ? 
O9 Cu2 Al 129.2(4) . 2_667 ? 
O2 Cu2 Al 81.1(4) . 2_667 ? 
O6 Cu2 Al 131.8(3) 2_656 2_667 ? 
O3 Cu2 Al 42.3(3) 1_556 2_667 ? 
Cu2 Cu2 Al 60.71(10) 2_657 2_667 ? 
As1 Cu2 Al 64.74(8) . 2_667 ? 
Fe Cu2 Al 56.15(11) 1_445 2_667 ? 
Al Cu2 Al 56.15(11) 1_445 2_667 ? 
Cu Cu2 Al 56.15(11) 1_445 2_667 ? 
Fe Cu2 Al 126.46(9) 1_545 2_667 ? 
Al Cu2 Al 126.46(9) 1_545 2_667 ? 
Cu Cu2 Al 126.46(9) 1_545 2_667 ? 
As1 Cu2 Al 135.25(10) 1_655 2_667 ? 
Fe Cu2 Al 0.00(14) 2_667 2_667 ? 
O7 Cu2 Cu 96.3(4) 2_657 2_667 ? 
O7 Cu2 Cu 35.5(4) . 2_667 ? 
O9 Cu2 Cu 129.2(4) . 2_667 ? 
O2 Cu2 Cu 81.1(4) . 2_667 ? 
O6 Cu2 Cu 131.8(3) 2_656 2_667 ? 
O3 Cu2 Cu 42.3(3) 1_556 2_667 ? 
Cu2 Cu2 Cu 60.71(10) 2_657 2_667 ? 
As1 Cu2 Cu 64.74(8) . 2_667 ? 
Fe Cu2 Cu 56.15(11) 1_445 2_667 ? 
Al Cu2 Cu 56.15(11) 1_445 2_667 ? 
Cu Cu2 Cu 56.15(11) 1_445 2_667 ? 
Fe Cu2 Cu 126.46(9) 1_545 2_667 ? 
Al Cu2 Cu 126.46(9) 1_545 2_667 ? 
Cu Cu2 Cu 126.46(9) 1_545 2_667 ? 
As1 Cu2 Cu 135.25(10) 1_655 2_667 ? 
Fe Cu2 Cu 0.00(14) 2_667 2_667 ? 
Al Cu2 Cu 0.00(14) 2_667 2_667 ? 
O7 Cu2 O1 106.8(4) 2_657 2_556 ? 
O7 Cu2 O1 56.7(4) . 2_556 ? 
O9 Cu2 O1 137.1(4) . 2_556 ? 
O2 Cu2 O1 63.1(4) . 2_556 ? 
O6 Cu2 O1 53.2(4) 2_656 2_556 ? 
O3 Cu2 O1 111.1(4) 1_556 2_556 ? 
Cu2 Cu2 O1 79.5(2) 2_657 2_556 ? 
As1 Cu2 O1 92.0(2) . 2_556 ? 
Fe Cu2 O1 33.6(2) 1_445 2_556 ? 
Al Cu2 O1 33.6(2) 1_445 2_556 ? 
Cu Cu2 O1 33.6(2) 1_445 2_556 ? 
Fe Cu2 O1 84.1(2) 1_545 2_556 ? 
Al Cu2 O1 84.1(2) 1_545 2_556 ? 
Cu Cu2 O1 84.1(2) 1_545 2_556 ? 
As1 Cu2 O1 137.3(2) 1_655 2_556 ? 
Fe Cu2 O1 86.4(2) 2_667 2_556 ? 
Al Cu2 O1 86.4(2) 2_667 2_556 ? 
Cu Cu2 O1 86.4(2) 2_667 2_556 ? 
O7 Cu2 As2 89.3(4) 2_657 2_656 ? 
O7 Cu2 As2 76.3(4) . 2_656 ? 
O9 Cu2 As2 119.3(4) . 2_656 ? 
O2 Cu2 As2 82.2(4) . 2_656 ? 
O6 Cu2 As2 25.0(3) 2_656 2_656 ? 
O3 Cu2 As2 139.1(3) 1_556 2_656 ? 
Cu2 Cu2 As2 80.06(10) 2_657 2_656 ? 
As1 Cu2 As2 114.98(9) . 2_656 ? 
Fe Cu2 As2 61.67(8) 1_445 2_656 ? 
Al Cu2 As2 61.67(8) 1_445 2_656 ? 
Cu Cu2 As2 61.67(8) 1_445 2_656 ? 
Fe Cu2 As2 58.30(8) 1_545 2_656 ? 
Al Cu2 As2 58.30(8) 1_545 2_656 ? 
Cu Cu2 As2 58.30(8) 1_545 2_656 ? 
As1 Cu2 As2 110.15(8) 1_655 2_656 ? 
Fe Cu2 As2 110.51(9) 2_667 2_656 ? 
Al Cu2 As2 110.51(9) 2_667 2_656 ? 
Cu Cu2 As2 110.51(9) 2_667 2_656 ? 
O1 Cu2 As2 28.2(2) 2_556 2_656 ? 
O6 Cu O1 92.8(6) 2_666 2_666 ? 
O6 Cu O7 167.2(5) 2_666 1_665 ? 
O1 Cu O7 97.7(6) 2_666 1_665 ? 
O6 Cu O7 88.1(5) 2_666 2_667 ? 
O1 Cu O7 174.8(5) 2_666 2_667 ? 
O7 Cu O7 82.0(5) 1_665 2_667 ? 
O6 Cu O3 100.1(5) 2_666 2_666 ? 
O1 Cu O3 84.0(5) 2_666 2_666 ? 
O7 Cu O3 88.3(5) 1_665 2_666 ? 
O7 Cu O3 90.8(5) 2_667 2_666 ? 
O6 Cu O2 94.8(5) 2_666 1_665 ? 
O1 Cu O2 93.9(5) 2_666 1_665 ? 
O7 Cu O2 77.2(5) 1_665 1_665 ? 
O7 Cu O2 91.1(5) 2_667 1_665 ? 
O3 Cu O2 165.0(5) 2_666 1_665 ? 
O6 Cu Fe 128.1(4) 2_666 2_777 ? 
O1 Cu Fe 139.0(4) 2_666 2_777 ? 
O7 Cu Fe 41.5(4) 1_665 2_777 ? 
O7 Cu Fe 40.5(3) 2_667 2_777 ? 
O3 Cu Fe 89.4(4) 2_666 2_777 ? 
O2 Cu Fe 82.4(3) 1_665 2_777 ? 
O6 Cu Al 128.1(4) 2_666 2_777 ? 
O1 Cu Al 139.0(4) 2_666 2_777 ? 
O7 Cu Al 41.5(4) 1_665 2_777 ? 
O7 Cu Al 40.5(3) 2_667 2_777 ? 
O3 Cu Al 89.4(4) 2_666 2_777 ? 
O2 Cu Al 82.4(3) 1_665 2_777 ? 
Fe Cu Al 0.00(13) 2_777 2_777 ? 
O6 Cu Cu 128.1(4) 2_666 2_777 ? 
O1 Cu Cu 139.0(4) 2_666 2_777 ? 
O7 Cu Cu 41.5(4) 1_665 2_777 ? 
O7 Cu Cu 40.5(3) 2_667 2_777 ? 
O3 Cu Cu 89.4(4) 2_666 2_777 ? 
O2 Cu Cu 82.4(3) 1_665 2_777 ? 
Fe Cu Cu 0.00(13) 2_777 2_777 ? 
Al Cu Cu 0.00(13) 2_777 2_777 ? 
O6 Cu Cu2 135.6(4) 2_666 1_665 ? 
O1 Cu Cu2 85.8(4) 2_666 1_665 ? 
O7 Cu Cu2 38.9(4) 1_665 1_665 ? 
O7 Cu Cu2 97.1(4) 2_667 1_665 ? 
O3 Cu Cu2 123.7(3) 2_666 1_665 ? 
O2 Cu Cu2 41.3(3) 1_665 1_665 ? 
Fe Cu Cu2 64.73(11) 2_777 1_665 ? 
Al Cu Cu2 64.73(11) 2_777 1_665 ? 
Cu Cu Cu2 64.73(11) 2_777 1_665 ? 
O6 Cu Cu2 52.0(4) 2_666 1_565 ? 
O1 Cu Cu2 144.1(4) 2_666 1_565 ? 
O7 Cu Cu2 116.3(4) 1_665 1_565 ? 
O7 Cu Cu2 37.9(4) 2_667 1_565 ? 
O3 Cu Cu2 106.6(3) 2_666 1_565 ? 
O2 Cu Cu2 83.7(3) 1_665 1_565 ? 
Fe Cu Cu2 76.30(12) 2_777 1_565 ? 
Al Cu Cu2 76.30(12) 2_777 1_565 ? 
Cu Cu Cu2 76.30(12) 2_777 1_565 ? 
Cu2 Cu Cu2 113.39(11) 1_665 1_565 ? 
O6 Cu Cu1 84.9(4) 2_666 . ? 
O1 Cu Cu1 48.4(4) 2_666 . ? 
O7 Cu Cu1 107.6(4) 1_665 . ? 
O7 Cu Cu1 126.7(4) 2_667 . ? 
O3 Cu Cu1 39.5(3) 2_666 . ? 
O2 Cu Cu1 142.1(3) 1_665 . ? 
Fe Cu Cu1 126.77(16) 2_777 . ? 
Al Cu Cu1 126.77(16) 2_777 . ? 
Cu Cu Cu1 126.77(16) 2_777 . ? 
Cu2 Cu Cu1 123.56(11) 1_665 . ? 
Cu2 Cu Cu1 123.05(11) 1_565 . ? 
O6 Cu Cu2 83.6(4) 2_666 2_667 ? 
O1 Cu Cu2 139.8(4) 2_666 2_667 ? 
O7 Cu Cu2 92.9(4) 1_665 2_667 ? 
O7 Cu Cu2 35.3(4) 2_667 2_667 ? 
O3 Cu Cu2 57.6(3) 2_666 2_667 ? 
O2 Cu Cu2 126.3(3) 1_665 2_667 ? 
Fe Cu Cu2 59.12(11) 2_777 2_667 ? 
Al Cu Cu2 59.12(11) 2_777 2_667 ? 
Cu Cu Cu2 59.12(11) 2_777 2_667 ? 
Cu2 Cu Cu2 123.85(10) 1_665 2_667 ? 
Cu2 Cu Cu2 53.54(9) 1_565 2_667 ? 
Cu1 Cu Cu2 91.44(10) . 2_667 ? 
O6 Cu As2 23.8(4) 2_666 2_666 ? 
O1 Cu As2 81.4(4) 2_666 2_666 ? 
O7 Cu As2 166.5(4) 1_665 2_666 ? 
O7 Cu As2 97.6(4) 2_667 2_666 ? 
O3 Cu As2 78.2(3) 2_666 2_666 ? 
O2 Cu As2 116.2(3) 1_665 2_666 ? 
Fe Cu As2 136.58(16) 2_777 2_666 ? 
Al Cu As2 136.58(16) 2_777 2_666 ? 
Cu Cu As2 136.58(16) 2_777 2_666 ? 
Cu2 Cu As2 153.26(12) 1_665 2_666 ? 
Cu2 Cu As2 68.06(8) 1_565 2_666 ? 
Cu1 Cu As2 61.78(8) . 2_666 ? 
Cu2 Cu As2 79.60(9) 2_667 2_666 ? 
O6 Cu As1 123.3(4) 2_666 2_667 ? 
O1 Cu As1 97.4(4) 2_666 2_667 ? 
O7 Cu As1 62.6(4) 1_665 2_667 ? 
O7 Cu As1 77.9(4) 2_667 2_667 ? 
O3 Cu As1 27.6(3) 2_666 2_667 ? 
O2 Cu As1 139.4(3) 1_665 2_667 ? 
Fe Cu As1 63.78(11) 2_777 2_667 ? 
Al Cu As1 63.78(11) 2_777 2_667 ? 
Cu Cu As1 63.78(11) 2_777 2_667 ? 
Cu2 Cu As1 100.81(10) 1_665 2_667 ? 
Cu2 Cu As1 107.60(10) 1_565 2_667 ? 
Cu1 Cu As1 63.07(8) . 2_667 ? 
Cu2 Cu As1 54.29(7) 2_667 2_667 ? 
As2 Cu As1 104.01(9) 2_666 2_667 ? 
O6 Cu As1 90.0(4) 2_666 1_665 ? 
O1 Cu As1 122.7(4) 2_666 1_665 ? 
O7 Cu As1 78.2(4) 1_665 1_665 ? 
O7 Cu As1 62.3(4) 2_667 1_665 ? 
O3 Cu As1 151.1(4) 2_666 1_665 ? 
O2 Cu As1 29.0(3) 1_665 1_665 ? 
Fe Cu As1 63.57(11) 2_777 1_665 ? 
Al Cu As1 63.57(11) 2_777 1_665 ? 
Cu Cu As1 63.57(11) 2_777 1_665 ? 
Cu2 Cu As1 55.57(7) 1_665 1_665 ? 
Cu2 Cu As1 59.21(7) 1_565 1_665 ? 
Cu1 Cu As1 169.27(12) . 1_665 ? 
Cu2 Cu As1 97.34(9) 2_667 1_665 ? 
As2 Cu As1 113.70(10) 2_666 1_665 ? 
As1 Cu As1 127.35(10) 2_667 1_665 ? 
O6 Cu As2 108.8(4) 2_666 2_766 ? 
O1 Cu As2 19.8(4) 2_666 2_766 ? 
O7 Cu As2 80.2(4) 1_665 2_766 ? 
O7 Cu As2 161.8(4) 2_667 2_766 ? 
O3 Cu As2 92.5(3) 2_666 2_766 ? 
O2 Cu As2 81.2(3) 1_665 2_766 ? 
Fe Cu As2 121.63(15) 2_777 2_766 ? 
Al Cu As2 121.63(15) 2_777 2_766 ? 
Cu Cu As2 121.63(15) 2_777 2_766 ? 
Cu2 Cu As2 66.27(8) 1_665 2_766 ? 
Cu2 Cu As2 154.44(11) 1_565 2_766 ? 
Cu1 Cu As2 63.37(8) . 2_766 ? 
Cu2 Cu As2 149.71(11) 2_667 2_766 ? 
As2 Cu As2 100.57(9) 2_666 2_766 ? 
As1 Cu As2 97.23(9) 2_667 2_766 ? 
As1 Cu As2 109.82(9) 1_665 2_766 ? 
O6 Cu O8 52.4(4) 2_666 . ? 
O1 Cu O8 68.0(5) 2_666 . ? 
O7 Cu O8 139.0(4) 1_665 . ? 
O7 Cu O8 108.8(4) 2_667 . ? 
O3 Cu O8 53.1(4) 2_666 . ? 
O2 Cu O8 139.3(4) 1_665 . ? 
Fe Cu O8 135.3(3) 2_777 . ? 
Al Cu O8 135.3(3) 2_777 . ? 
Cu Cu O8 135.3(3) 2_777 . ? 
Cu2 Cu O8 153.6(3) 1_665 . ? 
Cu2 Cu O8 90.8(2) 1_565 . ? 
Cu1 Cu O8 34.1(2) . . ? 
Cu2 Cu O8 78.6(2) 2_667 . ? 
As2 Cu O8 28.7(2) 2_666 . ? 
As1 Cu O8 80.7(2) 2_667 . ? 
As1 Cu O8 142.4(2) 1_665 . ? 
As2 Cu O8 87.3(2) 2_766 . ? 
O6 Cu O2 117.5(4) 2_666 2_667 ? 
O1 Cu O2 126.0(4) 2_666 2_667 ? 
O7 Cu O2 61.3(4) 1_665 2_667 ? 
O7 Cu O2 49.4(4) 2_667 2_667 ? 
O3 Cu O2 49.3(4) 2_666 2_667 ? 
O2 Cu O2 123.8(3) 1_665 2_667 ? 
Fe Cu O2 41.4(2) 2_777 2_667 ? 
Al Cu O2 41.4(2) 2_777 2_667 ? 
Cu Cu O2 41.4(2) 2_777 2_667 ? 
Cu2 Cu O2 98.2(3) 1_665 2_667 ? 
Cu2 Cu O2 82.8(2) 1_565 2_667 ? 
Cu1 Cu O2 88.6(2) . 2_667 ? 
Cu2 Cu O2 34.4(2) 2_667 2_667 ? 
As2 Cu O2 108.3(2) 2_666 2_667 ? 
As1 Cu O2 28.8(2) 2_667 2_667 ? 
As1 Cu O2 102.1(2) 1_665 2_667 ? 
As2 Cu O2 122.8(2) 2_766 2_667 ? 
O8 Cu O2 95.2(3) . 2_667 ? 
O6 Cu O3 113.1(4) 2_666 1_666 ? 
O1 Cu O3 132.2(4) 2_666 1_666 ? 
O7 Cu O3 54.1(4) 1_665 1_666 ? 
O7 Cu O3 51.6(4) 2_667 1_666 ? 
O3 Cu O3 126.3(3) 2_666 1_666 ? 
O2 Cu O3 46.7(4) 1_665 1_666 ? 
Fe Cu O3 36.8(2) 2_777 1_666 ? 
Al Cu O3 36.8(2) 2_777 1_666 ? 
Cu Cu O3 36.8(2) 2_777 1_666 ? 
Cu2 Cu O3 47.4(2) 1_665 1_666 ? 
Cu2 Cu O3 68.8(2) 1_565 1_666 ? 
Cu1 Cu O3 160.9(2) . 1_666 ? 
Cu2 Cu O3 84.7(2) 2_667 1_666 ? 
As2 Cu O3 135.1(2) 2_666 1_666 ? 
As1 Cu O3 100.1(2) 2_667 1_666 ? 
As1 Cu O3 27.9(2) 1_665 1_666 ? 
As2 Cu O3 113.3(2) 2_766 1_666 ? 
O8 Cu O3 158.9(3) . 1_666 ? 
O2 Cu O3 77.6(3) 2_667 1_666 ? 
As2 O1 Fe 137.8(8) 1_455 2_666 ? 
As2 O1 Al 137.8(8) 1_455 2_666 ? 
Fe O1 Al 0.0(3) 2_666 2_666 ? 
As2 O1 Cu 137.8(8) 1_455 2_666 ? 
Fe O1 Cu 0.0(3) 2_666 2_666 ? 
Al O1 Cu 0.0(3) 2_666 2_666 ? 
As2 O1 Cu1 114.8(7) 1_455 2_666 ? 
Fe O1 Cu1 93.8(5) 2_666 2_666 ? 
Al O1 Cu1 93.8(5) 2_666 2_666 ? 
Cu O1 Cu1 93.8(5) 2_666 2_666 ? 
As2 O1 K1 95.3(5) 1_455 . ? 
Fe O1 K1 99.4(5) 2_666 . ? 
Al O1 K1 99.4(5) 2_666 . ? 
Cu O1 K1 99.4(5) 2_666 . ? 
Cu1 O1 K1 115.8(5) 2_666 . ? 
As2 O1 Cu2 77.6(5) 1_455 2_556 ? 
Fe O1 Cu2 60.7(4) 2_666 2_556 ? 
Al O1 Cu2 60.7(4) 2_666 2_556 ? 
Cu O1 Cu2 60.7(4) 2_666 2_556 ? 
Cu1 O1 Cu2 137.3(5) 2_666 2_556 ? 
K1 O1 Cu2 102.6(4) . 2_556 ? 
As2 O1 Cu2 80.0(5) 1_455 1_454 ? 
Fe O1 Cu2 65.8(4) 2_666 1_454 ? 
Al O1 Cu2 65.8(4) 2_666 1_454 ? 
Cu O1 Cu2 65.8(4) 2_666 1_454 ? 
Cu1 O1 Cu2 96.5(4) 2_666 1_454 ? 
K1 O1 Cu2 145.8(4) . 1_454 ? 
Cu2 O1 Cu2 43.18(17) 2_556 1_454 ? 
As2 O1 Cu1 46.7(4) 1_455 1_455 ? 
Fe O1 Cu1 158.8(5) 2_666 1_455 ? 
Al O1 Cu1 158.8(5) 2_666 1_455 ? 
Cu O1 Cu1 158.8(5) 2_666 1_455 ? 
Cu1 O1 Cu1 101.1(4) 2_666 1_455 ? 
K1 O1 Cu1 60.6(3) . 1_455 ? 
Cu2 O1 Cu1 114.2(3) 2_556 1_455 ? 
Cu2 O1 Cu1 126.4(3) 1_454 1_455 ? 
As2 O1 Cu 38.5(3) 1_455 2_566 ? 
Fe O1 Cu 100.2(5) 2_666 2_566 ? 
Al O1 Cu 100.2(5) 2_666 2_566 ? 
Cu O1 Cu 100.2(5) 2_666 2_566 ? 
Cu1 O1 Cu 122.5(4) 2_666 2_566 ? 
K1 O1 Cu 116.3(3) . 2_566 ? 
Cu2 O1 Cu 43.93(16) 2_556 2_566 ? 
Cu2 O1 Cu 44.32(15) 1_454 2_566 ? 
Cu1 O1 Cu 84.5(2) 1_455 2_566 ? 
As2 O1 Cu 115.7(6) 1_455 1_444 ? 
Fe O1 Cu 24.9(3) 2_666 1_444 ? 
Al O1 Cu 24.9(3) 2_666 1_444 ? 
Cu O1 Cu 24.9(3) 2_666 1_444 ? 
Cu1 O1 Cu 98.2(4) 2_666 1_444 ? 
K1 O1 Cu 118.3(4) . 1_444 ? 
Cu2 O1 Cu 44.31(17) 2_556 1_444 ? 
Cu2 O1 Cu 41.01(14) 1_454 1_444 ? 
Cu1 O1 Cu 158.5(3) 1_455 1_444 ? 
Cu O1 Cu 77.2(2) 2_566 1_444 ? 
As2 O1 Na1 74.9(4) 1_455 1_455 ? 
Fe O1 Na1 97.5(4) 2_666 1_455 ? 
Al O1 Na1 97.5(4) 2_666 1_455 ? 
Cu O1 Na1 97.5(4) 2_666 1_455 ? 
Cu1 O1 Na1 58.3(3) 2_666 1_455 ? 
K1 O1 Na1 162.5(5) . 1_455 ? 
Cu2 O1 Na1 89.6(3) 2_556 1_455 ? 
Cu2 O1 Na1 48.01(15) 1_454 1_455 ? 
Cu1 O1 Na1 103.1(3) 1_455 1_455 ? 
Cu O1 Na1 64.65(18) 2_566 1_455 ? 
Cu O1 Na1 79.2(2) 1_444 1_455 ? 
As1 O2 Cu2 106.2(7) . . ? 
As1 O2 Fe 109.4(7) . 1_445 ? 
Cu2 O2 Fe 88.4(5) . 1_445 ? 
As1 O2 Al 109.4(7) . 1_445 ? 
Cu2 O2 Al 88.4(5) . 1_445 ? 
Fe O2 Al 0.00(16) 1_445 1_445 ? 
As1 O2 Cu 109.4(7) . 1_445 ? 
Cu2 O2 Cu 88.4(5) . 1_445 ? 
Fe O2 Cu 0.00(16) 1_445 1_445 ? 
Al O2 Cu 0.00(16) 1_445 1_445 ? 
As1 O2 K1 96.8(6) . . ? 
Cu2 O2 K1 94.5(5) . . ? 
Fe O2 K1 151.7(5) 1_445 . ? 
Al O2 K1 151.7(5) 1_445 . ? 
Cu O2 K1 151.7(5) 1_445 . ? 
As1 O2 Cu 69.3(4) . 2_667 ? 
Cu2 O2 Cu 64.5(4) . 2_667 ? 
Fe O2 Cu 56.2(3) 1_445 2_667 ? 
Al O2 Cu 56.2(3) 1_445 2_667 ? 
Cu O2 Cu 56.2(3) 1_445 2_667 ? 
K1 O2 Cu 148.3(5) . 2_667 ? 
As1 O2 K1 132.4(6) . 2_556 ? 
Cu2 O2 K1 121.4(5) . 2_556 ? 
Fe O2 K1 73.7(3) 1_445 2_556 ? 
Al O2 K1 73.7(3) 1_445 2_556 ? 
Cu O2 K1 73.7(3) 1_445 2_556 ? 
K1 O2 K1 80.8(3) . 2_556 ? 
Cu O2 K1 129.8(4) 2_667 2_556 ? 
As1 O2 Cu2 60.1(4) . 1_455 ? 
Cu2 O2 Cu2 126.5(5) . 1_455 ? 
Fe O2 Cu2 56.7(3) 1_445 1_455 ? 
Al O2 Cu2 56.7(3) 1_445 1_455 ? 
Cu O2 Cu2 56.7(3) 1_445 1_455 ? 
K1 O2 Cu2 136.0(4) . 1_455 ? 
Cu O2 Cu2 62.5(2) 2_667 1_455 ? 
K1 O2 Cu2 88.9(3) 2_556 1_455 ? 
As1 O2 Na1 52.6(4) . 1_556 ? 
Cu2 O2 Na1 66.1(4) . 1_556 ? 
Fe O2 Na1 137.2(5) 1_445 1_556 ? 
Al O2 Na1 137.2(5) 1_445 1_556 ? 
Cu O2 Na1 137.2(5) 1_445 1_556 ? 
K1 O2 Na1 68.1(3) . 1_556 ? 
Cu O2 Na1 81.3(3) 2_667 1_556 ? 
K1 O2 Na1 148.8(4) 2_556 1_556 ? 
Cu2 O2 Na1 111.1(3) 1_455 1_556 ? 
As1 O2 Cu1 40.9(3) . 1_455 ? 
Cu2 O2 Cu1 123.1(5) . 1_455 ? 
Fe O2 Cu1 138.4(5) 1_445 1_455 ? 
Al O2 Cu1 138.4(5) 1_445 1_455 ? 
Cu O2 Cu1 138.4(5) 1_445 1_455 ? 
K1 O2 Cu1 60.3(3) . 1_455 ? 
Cu O2 Cu1 110.1(3) 2_667 1_455 ? 
K1 O2 Cu1 104.8(3) 2_556 1_455 ? 
Cu2 O2 Cu1 81.9(3) 1_455 1_455 ? 
Na1 O2 Cu1 57.38(18) 1_556 1_455 ? 
As1 O2 Cu2 108.1(5) . 2_657 ? 
Cu2 O2 Cu2 30.8(3) . 2_657 ? 
Fe O2 Cu2 58.4(3) 1_445 2_657 ? 
Al O2 Cu2 58.4(3) 1_445 2_657 ? 
Cu O2 Cu2 58.4(3) 1_445 2_657 ? 
K1 O2 Cu2 123.7(4) . 2_657 ? 
Cu O2 Cu2 44.23(16) 2_667 2_657 ? 
K1 O2 Cu2 112.4(3) 2_556 2_657 ? 
Cu2 O2 Cu2 99.8(3) 1_455 2_657 ? 
Na1 O2 Cu2 88.4(3) 1_556 2_657 ? 
Cu1 O2 Cu2 142.8(3) 1_455 2_657 ? 
As1 O3 Cu1 130.4(8) 1_554 2_666 ? 
As1 O3 Fe 116.0(7) 1_554 2_666 ? 
Cu1 O3 Fe 96.6(5) 2_666 2_666 ? 
As1 O3 Al 116.0(7) 1_554 2_666 ? 
Cu1 O3 Al 96.6(5) 2_666 2_666 ? 
Fe O3 Al 0.00(17) 2_666 2_666 ? 
As1 O3 Cu 116.0(7) 1_554 2_666 ? 
Cu1 O3 Cu 96.6(5) 2_666 2_666 ? 
Fe O3 Cu 0.00(17) 2_666 2_666 ? 
Al O3 Cu 0.00(17) 2_666 2_666 ? 
As1 O3 Cu2 80.1(5) 1_554 1_554 ? 
Cu1 O3 Cu2 145.0(6) 2_666 1_554 ? 
Fe O3 Cu2 80.1(4) 2_666 1_554 ? 
Al O3 Cu2 80.1(4) 2_666 1_554 ? 
Cu O3 Cu2 80.1(4) 2_666 1_554 ? 
As1 O3 Na1 83.9(5) 1_554 . ? 
Cu1 O3 Na1 86.5(5) 2_666 . ? 
Fe O3 Na1 148.4(6) 2_666 . ? 
Al O3 Na1 148.4(6) 2_666 . ? 
Cu O3 Na1 148.4(6) 2_666 . ? 
Cu2 O3 Na1 79.5(3) 1_554 . ? 
As1 O3 Cu 65.3(4) 1_554 1_444 ? 
Cu1 O3 Cu 146.2(6) 2_666 1_444 ? 
Fe O3 Cu 53.7(3) 2_666 1_444 ? 
Al O3 Cu 53.7(3) 2_666 1_444 ? 
Cu O3 Cu 53.7(3) 2_666 1_444 ? 
Cu2 O3 Cu 54.6(2) 1_554 1_444 ? 
Na1 O3 Cu 127.1(4) . 1_444 ? 
As1 O3 Cu2 54.8(4) 1_554 1_454 ? 
Cu1 O3 Cu2 111.1(5) 2_666 1_454 ? 
Fe O3 Cu2 70.4(3) 2_666 1_454 ? 
Al O3 Cu2 70.4(3) 2_666 1_454 ? 
Cu O3 Cu2 70.4(3) 2_666 1_454 ? 
Cu2 O3 Cu2 100.7(4) 1_554 1_454 ? 
Na1 O3 Cu2 137.4(4) . 1_454 ? 
Cu O3 Cu2 48.36(17) 1_444 1_454 ? 
As1 O3 Na1 58.8(4) 1_554 1_455 ? 
Cu1 O3 Na1 74.6(4) 2_666 1_455 ? 
Fe O3 Na1 113.6(4) 2_666 1_455 ? 
Al O3 Na1 113.6(4) 2_666 1_455 ? 
Cu O3 Na1 113.6(4) 2_666 1_455 ? 
Cu2 O3 Na1 138.8(4) 1_554 1_455 ? 
Na1 O3 Na1 97.6(4) . 1_455 ? 
Cu O3 Na1 100.9(3) 1_444 1_455 ? 
Cu2 O3 Na1 54.53(17) 1_454 1_455 ? 
As1 O3 Cu2 112.7(5) 1_554 2_656 ? 
Cu1 O3 Cu2 116.7(5) 2_666 2_656 ? 
Fe O3 Cu2 43.8(3) 2_666 2_656 ? 
Al O3 Cu2 43.8(3) 2_666 2_656 ? 
Cu O3 Cu2 43.8(3) 2_666 2_656 ? 
Cu2 O3 Cu2 41.1(2) 1_554 2_656 ? 
Na1 O3 Cu2 107.1(3) . 2_656 ? 
Cu O3 Cu2 55.5(2) 1_444 2_656 ? 
Cu2 O3 Cu2 99.0(3) 1_454 2_656 ? 
Na1 O3 Cu2 153.0(4) 1_455 2_656 ? 
As2 O4 Cu1 132.1(8) 2_666 2_666 ? 
As2 O4 K1 103.1(6) 2_666 2_566 ? 
Cu1 O4 K1 106.9(6) 2_666 2_566 ? 
As2 O4 K1 97.0(6) 2_666 2_666 ? 
Cu1 O4 K1 90.0(5) 2_666 2_666 ? 
K1 O4 K1 131.7(5) 2_566 2_666 ? 
As2 O4 Cu1 42.7(4) 2_666 . ? 
Cu1 O4 Cu1 96.0(5) 2_666 . ? 
K1 O4 Cu1 144.2(4) 2_566 . ? 
K1 O4 Cu1 73.9(3) 2_666 . ? 
As2 O4 Cu1 48.0(4) 2_666 1_455 ? 
Cu1 O4 Cu1 106.7(5) 2_666 1_455 ? 
K1 O4 Cu1 74.6(3) 2_566 1_455 ? 
K1 O4 Cu1 143.8(4) 2_666 1_455 ? 
Cu1 O4 Cu1 72.6(2) . 1_455 ? 
As2 O4 Cu 39.6(4) 2_666 . ? 
Cu1 O4 Cu 130.6(6) 2_666 . ? 
K1 O4 Cu 122.5(4) 2_566 . ? 
K1 O4 Cu 58.1(3) 2_666 . ? 
Cu1 O4 Cu 42.58(14) . . ? 
Cu1 O4 Cu 87.5(2) 1_455 . ? 
As2 O4 Cu 45.0(4) 2_666 1_455 ? 
Cu1 O4 Cu 146.0(6) 2_666 1_455 ? 
K1 O4 Cu 58.3(3) 2_566 1_455 ? 
K1 O4 Cu 123.2(4) 2_666 1_455 ? 
Cu1 O4 Cu 87.5(2) . 1_455 ? 
Cu1 O4 Cu 42.36(13) 1_455 1_455 ? 
Cu O4 Cu 71.8(2) . 1_455 ? 
As2 O4 Cu2 43.0(4) 2_666 1_565 ? 
Cu1 O4 Cu2 170.8(6) 2_666 1_565 ? 
K1 O4 Cu2 82.4(3) 2_566 1_565 ? 
K1 O4 Cu2 83.4(3) 2_666 1_565 ? 
Cu1 O4 Cu2 75.9(2) . 1_565 ? 
Cu1 O4 Cu2 75.6(2) 1_455 1_565 ? 
Cu O4 Cu2 40.18(13) . 1_565 ? 
Cu O4 Cu2 39.78(12) 1_455 1_565 ? 
As2 O4 Na1 142.8(6) 2_666 . ? 
Cu1 O4 Na1 38.3(3) 2_666 . ? 
K1 O4 Na1 114.1(4) 2_566 . ? 
K1 O4 Na1 56.3(2) 2_666 . ? 
Cu1 O4 Na1 101.0(3) . . ? 
Cu1 O4 Na1 144.6(3) 1_455 . ? 
Cu O4 Na1 111.6(3) . . ? 
Cu O4 Na1 170.5(3) 1_455 . ? 
Cu2 O4 Na1 138.0(3) 1_565 . ? 
As2 O4 K1 61.9(4) 2_666 . ? 
Cu1 O4 K1 71.3(4) 2_666 . ? 
K1 O4 K1 117.2(4) 2_566 . ? 
K1 O4 K1 111.0(4) 2_666 . ? 
Cu1 O4 K1 45.24(14) . . ? 
Cu1 O4 K1 49.44(15) 1_455 . ? 
Cu O4 K1 85.3(2) . . ? 
Cu O4 K1 88.2(2) 1_455 . ? 
Cu2 O4 K1 104.9(3) 1_565 . ? 
Na1 O4 K1 100.9(3) . . ? 
As2 O4 K1 90.2(5) 2_666 1_565 ? 
Cu1 O4 K1 136.4(5) 2_666 1_565 ? 
K1 O4 K1 64.8(3) 2_566 1_565 ? 
K1 O4 K1 71.8(3) 2_666 1_565 ? 
Cu1 O4 K1 115.2(3) . 1_565 ? 
Cu1 O4 K1 111.2(3) 1_455 1_565 ? 
Cu O4 K1 72.6(2) . 1_565 ? 
Cu O4 K1 69.0(2) 1_455 1_565 ? 
Cu2 O4 K1 47.12(15) 1_565 1_565 ? 
Na1 O4 K1 103.1(3) . 1_565 ? 
K1 O4 K1 152.0(3) . 1_565 ? 
As1 O5 Cu1 120.9(7) . 1_455 ? 
As1 O5 Ca1 103.1(5) . 1_556 ? 
Cu1 O5 Ca1 132.6(6) 1_455 1_556 ? 
As1 O5 Na1 103.1(5) . 1_556 ? 
Cu1 O5 Na1 132.6(6) 1_455 1_556 ? 
Ca1 O5 Na1 0.0 1_556 1_556 ? 
As1 O5 K1 97.0(6) . . ? 
Cu1 O5 K1 97.5(5) 1_455 . ? 
Ca1 O5 K1 93.8(4) 1_556 . ? 
Na1 O5 K1 93.8(4) 1_556 . ? 
As1 O5 Na1 69.2(4) . 1_456 ? 
Cu1 O5 Na1 67.2(4) 1_455 1_456 ? 
Ca1 O5 Na1 119.3(5) 1_556 1_456 ? 
Na1 O5 Na1 119.3(5) 1_556 1_456 ? 
K1 O5 Na1 145.9(4) . 1_456 ? 
As1 O5 Cu2 50.6(3) . . ? 
Cu1 O5 Cu2 156.9(6) 1_455 . ? 
Ca1 O5 Cu2 67.1(3) 1_556 . ? 
Na1 O5 Cu2 67.1(3) 1_556 . ? 
K1 O5 Cu2 65.7(3) . . ? 
Na1 O5 Cu2 117.4(3) 1_456 . ? 
As1 O5 Cu1 62.5(4) . 2_667 ? 
Cu1 O5 Cu1 123.9(6) 1_455 2_667 ? 
Ca1 O5 Cu1 60.6(3) 1_556 2_667 ? 
Na1 O5 Cu1 60.6(3) 1_556 2_667 ? 
K1 O5 Cu1 138.5(4) . 2_667 ? 
Na1 O5 Cu1 63.6(2) 1_456 2_667 ? 
Cu2 O5 Cu1 74.0(2) . 2_667 ? 
As1 O5 K1 70.5(4) . 1_455 ? 
Cu1 O5 K1 53.3(3) 1_455 1_455 ? 
Ca1 O5 K1 173.5(5) 1_556 1_455 ? 
Na1 O5 K1 173.5(5) 1_556 1_455 ? 
K1 O5 K1 87.7(3) . 1_455 ? 
Na1 O5 K1 58.55(19) 1_456 1_455 ? 
Cu2 O5 K1 107.9(3) . 1_455 ? 
Cu1 O5 K1 114.6(3) 2_667 1_455 ? 
As1 O5 Cu1 130.7(6) . . ? 
Cu1 O5 Cu1 103.2(4) 1_455 . ? 
Ca1 O5 Cu1 50.7(3) 1_556 . ? 
Na1 O5 Cu1 50.7(3) 1_556 . ? 
K1 O5 Cu1 53.5(2) . . ? 
Na1 O5 Cu1 156.6(4) 1_456 . ? 
Cu2 O5 Cu1 80.2(2) . . ? 
Cu1 O5 Cu1 111.3(3) 2_667 . ? 
K1 O5 Cu1 133.9(3) 1_455 . ? 
As1 O5 Cu 141.9(6) . 1_455 ? 
Cu1 O5 Cu 38.2(3) 1_455 1_455 ? 
Ca1 O5 Cu 95.8(4) 1_556 1_455 ? 
Na1 O5 Cu 95.8(4) 1_556 1_455 ? 
K1 O5 Cu 114.7(3) . 1_455 ? 
Na1 O5 Cu 72.7(2) 1_456 1_455 ? 
Cu2 O5 Cu 162.6(3) . 1_455 ? 
Cu1 O5 Cu 100.8(3) 2_667 1_455 ? 
K1 O5 Cu 89.4(2) 1_455 1_455 ? 
Cu1 O5 Cu 86.7(2) . 1_455 ? 
As1 O5 Cu2 24.9(3) . 1_455 ? 
Cu1 O5 Cu2 96.3(4) 1_455 1_455 ? 
Ca1 O5 Cu2 124.3(4) 1_556 1_455 ? 
Na1 O5 Cu2 124.3(4) 1_556 1_455 ? 
K1 O5 Cu2 106.1(4) . 1_455 ? 
Na1 O5 Cu2 49.59(16) 1_456 1_455 ? 
Cu2 O5 Cu2 74.8(2) . 1_455 ? 
Cu1 O5 Cu2 71.0(2) 2_667 1_455 ? 
K1 O5 Cu2 49.28(15) 1_455 1_455 ? 
Cu1 O5 Cu2 153.1(3) . 1_455 ? 
Cu O5 Cu2 119.7(3) 1_455 1_455 ? 
As2 O6 Fe 129.3(8) . 2_666 ? 
As2 O6 Al 129.3(8) . 2_666 ? 
Fe O6 Al 0.00(11) 2_666 2_666 ? 
As2 O6 Cu 129.3(8) . 2_666 ? 
Fe O6 Cu 0.00(11) 2_666 2_666 ? 
Al O6 Cu 0.00(11) 2_666 2_666 ? 
As2 O6 Cu2 117.6(6) . 2_656 ? 
Fe O6 Cu2 89.8(5) 2_666 2_656 ? 
Al O6 Cu2 89.8(5) 2_666 2_656 ? 
Cu O6 Cu2 89.8(5) 2_666 2_656 ? 
As2 O6 K1 90.5(5) . . ? 
Fe O6 K1 95.4(5) 2_666 . ? 
Al O6 K1 95.4(5) 2_666 . ? 
Cu O6 K1 95.4(5) 2_666 . ? 
Cu2 O6 K1 138.1(5) 2_656 . ? 
As2 O6 Cu1 67.7(4) . 2_666 ? 
Fe O6 Cu1 62.7(4) 2_666 2_666 ? 
Al O6 Cu1 62.7(4) 2_666 2_666 ? 
Cu O6 Cu1 62.7(4) 2_666 2_666 ? 
Cu2 O6 Cu1 132.6(5) 2_656 2_666 ? 
K1 O6 Cu1 85.2(3) . 2_666 ? 
As2 O6 Cu2 98.0(5) . 1_554 ? 
Fe O6 Cu2 64.2(4) 2_666 1_554 ? 
Al O6 Cu2 64.2(4) 2_666 1_554 ? 
Cu O6 Cu2 64.2(4) 2_666 1_554 ? 
Cu2 O6 Cu2 52.7(3) 2_656 1_554 ? 
K1 O6 Cu2 158.8(5) . 1_554 ? 
Cu1 O6 Cu2 80.1(3) 2_666 1_554 ? 
As2 O6 Cu 64.1(4) . 2_766 ? 
Fe O6 Cu 125.0(5) 2_666 2_766 ? 
Al O6 Cu 125.0(5) 2_666 2_766 ? 
Cu O6 Cu 125.0(5) 2_666 2_766 ? 
Cu2 O6 Cu 53.6(3) 2_656 2_766 ? 
K1 O6 Cu 139.6(4) . 2_766 ? 
Cu1 O6 Cu 110.3(3) 2_666 2_766 ? 
Cu2 O6 Cu 60.9(2) 1_554 2_766 ? 
As2 O6 K1 110.3(6) . 2_656 ? 
Fe O6 K1 120.4(5) 2_666 2_656 ? 
Al O6 K1 120.4(5) 2_666 2_656 ? 
Cu O6 K1 120.4(5) 2_666 2_656 ? 
Cu2 O6 K1 62.3(3) 2_656 2_656 ? 
K1 O6 K1 79.6(3) . 2_656 ? 
Cu1 O6 K1 164.8(4) 2_666 2_656 ? 
Cu2 O6 K1 114.9(3) 1_554 2_656 ? 
Cu O6 K1 80.7(3) 2_766 2_656 ? 
As2 O6 K1 49.5(4) . 1_655 ? 
Fe O6 K1 178.6(5) 2_666 1_655 ? 
Al O6 K1 178.6(5) 2_666 1_655 ? 
Cu O6 K1 178.6(5) 2_666 1_655 ? 
Cu2 O6 K1 90.4(4) 2_656 1_655 ? 
K1 O6 K1 85.4(3) . 1_655 ? 
Cu1 O6 K1 116.3(3) 2_666 1_655 ? 
Cu2 O6 K1 114.8(3) 1_554 1_655 ? 
Cu O6 K1 54.17(19) 2_766 1_655 ? 
K1 O6 K1 60.9(2) 2_656 1_655 ? 
As2 O6 Cu 138.2(6) . 1_444 ? 
Fe O6 Cu 31.9(3) 2_666 1_444 ? 
Al O6 Cu 31.9(3) 2_666 1_444 ? 
Cu O6 Cu 31.9(3) 2_666 1_444 ? 
Cu2 O6 Cu 58.0(3) 2_656 1_444 ? 
K1 O6 Cu 120.5(4) . 1_444 ? 
Cu1 O6 Cu 86.4(3) 2_666 1_444 ? 
Cu2 O6 Cu 43.62(16) 1_554 1_444 ? 
Cu O6 Cu 98.2(3) 2_766 1_444 ? 
K1 O6 Cu 102.9(3) 2_656 1_444 ? 
K1 O6 Cu 148.0(3) 1_655 1_444 ? 
Fe O7 Al 0.00(18) 1_445 1_445 ? 
Fe O7 Cu 0.00(18) 1_445 1_445 ? 
Al O7 Cu 0.00(18) 1_445 1_445 ? 
Fe O7 Cu2 147.5(7) 1_445 2_657 ? 
Al O7 Cu2 147.5(7) 1_445 2_657 ? 
Cu O7 Cu2 147.5(7) 1_445 2_657 ? 
Fe O7 Cu2 102.9(5) 1_445 . ? 
Al O7 Cu2 102.9(5) 1_445 . ? 
Cu O7 Cu2 102.9(5) 1_445 . ? 
Cu2 O7 Cu2 93.0(5) 2_657 . ? 
Fe O7 Fe 98.0(5) 1_445 2_667 ? 
Al O7 Fe 98.0(5) 1_445 2_667 ? 
Cu O7 Fe 98.0(5) 1_445 2_667 ? 
Cu2 O7 Fe 103.3(5) 2_657 2_667 ? 
Cu2 O7 Fe 109.2(6) . 2_667 ? 
Fe O7 Al 98.0(5) 1_445 2_667 ? 
Al O7 Al 98.0(5) 1_445 2_667 ? 
Cu O7 Al 98.0(5) 1_445 2_667 ? 
Cu2 O7 Al 103.3(5) 2_657 2_667 ? 
Cu2 O7 Al 109.2(6) . 2_667 ? 
Fe O7 Al 0.00(18) 2_667 2_667 ? 
Fe O7 Cu 98.0(5) 1_445 2_667 ? 
Al O7 Cu 98.0(5) 1_445 2_667 ? 
Cu O7 Cu 98.0(5) 1_445 2_667 ? 
Cu2 O7 Cu 103.3(5) 2_657 2_667 ? 
Cu2 O7 Cu 109.2(6) . 2_667 ? 
Fe O7 Cu 0.00(18) 2_667 2_667 ? 
Al O7 Cu 0.00(18) 2_667 2_667 ? 
Fe O7 Cu2 56.8(3) 1_445 2_557 ? 
Al O7 Cu2 56.8(3) 1_445 2_557 ? 
Cu O7 Cu2 56.8(3) 1_445 2_557 ? 
Cu2 O7 Cu2 121.2(5) 2_657 2_557 ? 
Cu2 O7 Cu2 142.6(5) . 2_557 ? 
Fe O7 Cu2 52.1(3) 2_667 2_557 ? 
Al O7 Cu2 52.1(3) 2_667 2_557 ? 
Cu O7 Cu2 52.1(3) 2_667 2_557 ? 
Fe O7 Cu 117.3(5) 1_445 1_545 ? 
Al O7 Cu 117.3(5) 1_445 1_545 ? 
Cu O7 Cu 117.3(5) 1_445 1_545 ? 
Cu2 O7 Cu 54.3(3) 2_657 1_545 ? 
Cu2 O7 Cu 50.2(3) . 1_545 ? 
Fe O7 Cu 141.3(5) 2_667 1_545 ? 
Al O7 Cu 141.3(5) 2_667 1_545 ? 
Cu O7 Cu 141.3(5) 2_667 1_545 ? 
Cu2 O7 Cu 164.0(4) 2_557 1_545 ? 
Fe O7 Cu1 46.1(3) 1_445 1_445 ? 
Al O7 Cu1 46.1(3) 1_445 1_445 ? 
Cu O7 Cu1 46.1(3) 1_445 1_445 ? 
Cu2 O7 Cu1 101.5(4) 2_657 1_445 ? 
Cu2 O7 Cu1 121.8(5) . 1_445 ? 
Fe O7 Cu1 121.1(5) 2_667 1_445 ? 
Al O7 Cu1 121.1(5) 2_667 1_445 ? 
Cu O7 Cu1 121.1(5) 2_667 1_445 ? 
Cu2 O7 Cu1 69.27(19) 2_557 1_445 ? 
Cu O7 Cu1 95.9(3) 1_545 1_445 ? 
Fe O7 Cu2 39.9(3) 1_445 1_455 ? 
Al O7 Cu2 39.9(3) 1_445 1_455 ? 
Cu O7 Cu2 39.9(3) 1_445 1_455 ? 
Cu2 O7 Cu2 159.7(5) 2_657 1_455 ? 
Cu2 O7 Cu2 103.2(4) . 1_455 ? 
Fe O7 Cu2 59.9(3) 2_667 1_455 ? 
Al O7 Cu2 59.9(3) 2_667 1_455 ? 
Cu O7 Cu2 59.9(3) 2_667 1_455 ? 
Cu2 O7 Cu2 40.29(13) 2_557 1_455 ? 
Cu O7 Cu2 146.0(3) 1_545 1_455 ? 
Cu1 O7 Cu2 80.5(2) 1_445 1_455 ? 
As2 O8 Cu1 128.4(7) 2_666 . ? 
As2 O8 K1 135.9(6) 2_666 . ? 
Cu1 O8 K1 92.0(5) . . ? 
As2 O8 Na1 124.1(6) 2_666 1_556 ? 
Cu1 O8 Na1 74.3(4) . 1_556 ? 
K1 O8 Na1 78.8(3) . 1_556 ? 
As2 O8 Cu1 78.1(5) 2_666 1_455 ? 
Cu1 O8 Cu1 145.3(5) . 1_455 ? 
K1 O8 Cu1 75.0(3) . 1_455 ? 
Na1 O8 Cu1 71.6(3) 1_556 1_455 ? 
As2 O8 Cu 68.1(4) 2_666 . ? 
Cu1 O8 Cu 63.7(3) . . ? 
K1 O8 Cu 155.5(5) . . ? 
Na1 O8 Cu 90.5(3) 1_556 . ? 
Cu1 O8 Cu 122.6(4) 1_455 . ? 
As2 O8 Cu1 63.0(4) 2_666 2_666 ? 
Cu1 O8 Cu1 116.2(5) . 2_666 ? 
K1 O8 Cu1 85.2(3) . 2_666 ? 
Na1 O8 Cu1 161.3(4) 1_556 2_666 ? 
Cu1 O8 Cu1 95.1(3) 1_455 2_666 ? 
Cu O8 Cu1 107.9(3) . 2_666 ? 
As2 O8 K1 54.0(4) 2_666 2_666 ? 
Cu1 O8 K1 84.2(4) . 2_666 ? 
K1 O8 K1 127.5(4) . 2_666 ? 
Na1 O8 K1 147.1(4) 1_556 2_666 ? 
Cu1 O8 K1 129.3(4) 1_455 2_666 ? 
Cu O8 K1 57.3(2) . 2_666 ? 
Cu1 O8 K1 51.57(18) 2_666 2_666 ? 
As2 O8 Cu2 74.9(5) 2_666 2_667 ? 
Cu1 O8 Cu2 86.1(4) . 2_667 ? 
K1 O8 Cu2 132.0(4) . 2_667 ? 
Na1 O8 Cu2 54.5(2) 1_556 2_667 ? 
Cu1 O8 Cu2 79.8(3) 1_455 2_667 ? 
Cu O8 Cu2 47.94(18) . 2_667 ? 
Cu1 O8 Cu2 137.7(3) 2_666 2_667 ? 
K1 O8 Cu2 100.1(3) 2_666 2_667 ? 
As2 O8 Cu 43.4(4) 2_666 1_455 ? 
Cu1 O8 Cu 136.4(5) . 1_455 ? 
K1 O8 Cu 120.1(4) . 1_455 ? 
Na1 O8 Cu 83.5(3) 1_556 1_455 ? 
Cu1 O8 Cu 45.15(18) 1_455 1_455 ? 
Cu O8 Cu 79.8(3) . 1_455 ? 
Cu1 O8 Cu 96.5(3) 2_666 1_455 ? 
K1 O8 Cu 96.0(3) 2_666 1_455 ? 
Cu2 O8 Cu 50.82(17) 2_667 1_455 ? 
As2 O8 Cu2 39.5(3) 2_666 1_565 ? 
Cu1 O8 Cu2 103.3(4) . 1_565 ? 
K1 O8 Cu2 158.3(4) . 1_565 ? 
Na1 O8 Cu2 90.6(3) 1_556 1_565 ? 
Cu1 O8 Cu2 83.8(3) 1_455 1_565 ? 
Cu O8 Cu2 41.15(16) . 1_565 ? 
Cu1 O8 Cu2 101.1(3) 2_666 1_565 ? 
K1 O8 Cu2 70.1(2) 2_666 1_565 ? 
Cu2 O8 Cu2 36.69(12) 2_667 1_565 ? 
Cu O8 Cu2 39.07(13) 1_455 1_565 ? 
As2 O8 K1 26.8(3) 2_666 2_566 ? 
Cu1 O8 K1 151.3(5) . 2_566 ? 
K1 O8 K1 109.2(3) . 2_566 ? 
Na1 O8 K1 127.6(4) 1_556 2_566 ? 
Cu1 O8 K1 61.8(2) 1_455 2_566 ? 
Cu O8 K1 94.8(3) . 2_566 ? 
Cu1 O8 K1 49.64(16) 2_666 2_566 ? 
K1 O8 K1 67.59(19) 2_666 2_566 ? 
Cu2 O8 K1 93.2(3) 2_667 2_566 ? 
Cu O8 K1 46.85(15) 1_455 2_566 ? 
Cu2 O8 K1 62.80(18) 1_565 2_566 ? 
As1 O9 Cu2 118.0(6) 1_655 . ? 
As1 O9 Ca1 111.0(6) 1_655 1_556 ? 
Cu2 O9 Ca1 108.2(5) . 1_556 ? 
As1 O9 Na1 111.0(6) 1_655 1_556 ? 
Cu2 O9 Na1 108.2(5) . 1_556 ? 
Ca1 O9 Na1 0.0 1_556 1_556 ? 
As1 O9 K1 123.1(6) 1_655 . ? 
Cu2 O9 K1 98.0(5) . . ? 
Ca1 O9 K1 95.6(4) 1_556 . ? 
Na1 O9 K1 95.6(4) 1_556 . ? 
As1 O9 Cu1 72.7(4) 1_655 . ? 
Cu2 O9 Cu1 167.2(6) . . ? 
Ca1 O9 Cu1 71.8(3) 1_556 . ? 
Na1 O9 Cu1 71.8(3) 1_556 . ? 
K1 O9 Cu1 69.5(3) . . ? 
As1 O9 Cu 65.4(4) 1_655 1_545 ? 
Cu2 O9 Cu 57.1(3) . 1_545 ? 
Ca1 O9 Cu 151.0(4) 1_556 1_545 ? 
Na1 O9 Cu 151.0(4) 1_556 1_545 ? 
K1 O9 Cu 110.5(4) . 1_545 ? 
Cu1 O9 Cu 128.5(4) . 1_545 ? 
As1 O9 Cu 55.5(3) 1_655 2_767 ? 
Cu2 O9 Cu 68.0(3) . 2_767 ? 
Ca1 O9 Cu 107.5(4) 1_556 2_767 ? 
Na1 O9 Cu 107.5(4) 1_556 2_767 ? 
K1 O9 Cu 155.7(4) . 2_767 ? 
Cu1 O9 Cu 124.5(4) . 2_767 ? 
Cu O9 Cu 45.25(16) 1_545 2_767 ? 
As1 O9 Cu1 54.1(3) 1_655 2_767 ? 
Cu2 O9 Cu1 102.6(4) . 2_767 ? 
Ca1 O9 Cu1 68.6(3) 1_556 2_767 ? 
Na1 O9 Cu1 68.6(3) 1_556 2_767 ? 
K1 O9 Cu1 157.1(4) . 2_767 ? 
Cu1 O9 Cu1 89.4(3) . 2_767 ? 
Cu O9 Cu1 89.2(3) 1_545 2_767 ? 
Cu O9 Cu1 45.90(14) 2_767 2_767 ? 
As1 O9 Cu2 22.7(3) 1_655 1_655 ? 
Cu2 O9 Cu2 97.0(4) . 1_655 ? 
Ca1 O9 Cu2 130.0(4) 1_556 1_655 ? 
Na1 O9 Cu2 130.0(4) 1_556 1_655 ? 
K1 O9 Cu2 123.3(4) . 1_655 ? 
Cu1 O9 Cu2 92.2(3) . 1_655 ? 
Cu O9 Cu2 42.63(14) 1_545 1_655 ? 
Cu O9 Cu2 44.26(14) 2_767 1_655 ? 
Cu1 O9 Cu2 64.10(18) 2_767 1_655 ? 
As1 O9 Cu2 94.4(4) 1_655 2_657 ? 
Cu2 O9 Cu2 26.4(2) . 2_657 ? 
Ca1 O9 Cu2 109.9(4) 1_556 2_657 ? 
Na1 O9 Cu2 109.9(4) 1_556 2_657 ? 
K1 O9 Cu2 123.1(4) . 2_657 ? 
Cu1 O9 Cu2 166.2(4) . 2_657 ? 
Cu O9 Cu2 45.05(14) 1_545 2_657 ? 
Cu O9 Cu2 41.70(12) 2_767 2_657 ? 
Cu1 O9 Cu2 78.9(2) 2_767 2_657 ? 
Cu2 O9 Cu2 76.20(19) 1_655 2_657 ? 
As1 O9 Na1 23.7(3) 1_655 1_656 ? 
Cu2 O9 Na1 135.7(5) . 1_656 ? 
Ca1 O9 Na1 88.4(3) 1_556 1_656 ? 
Na1 O9 Na1 88.4(3) 1_556 1_656 ? 
K1 O9 Na1 121.6(3) . 1_656 ? 
Cu1 O9 Na1 56.71(19) . 1_656 ? 
Cu O9 Na1 88.5(3) 1_545 1_656 ? 
Cu O9 Na1 67.85(19) 2_767 1_656 ? 
Cu1 O9 Na1 44.92(13) 2_767 1_656 ? 
Cu2 O9 Na1 46.14(13) 1_655 1_656 ? 
Cu2 O9 Na1 109.5(2) 2_657 1_656 ? 
 
_diffrn_measured_fraction_theta_max    0.999 
_diffrn_reflns_theta_full              28.28 
_diffrn_measured_fraction_theta_full   0.999 
_refine_diff_density_max    2.484 
_refine_diff_density_min   -1.967 
_refine_diff_density_rms    0.474 
